325 45 8MB
English Pages 341 Year 2002
Semiconductors for Micro and Nanotechnology— An Introduction for Engineers
Semiconductors for Micro and Nanotechnology— An Introduction for Engineers Jan G. Korvink and Andreas Greiner
Authors: Prof. Dr. Jan G. Korvink IMTEKInstitute for Microsystem Technology Faculty for Applied Sciences Albert Ludwig University Freiburg D79110 Freiburg Germany
Dr. Andreas Greiner IMTEKInstitute for Microsystem Technology Faculty for Applied Sciences Albert Ludwig University Freiburg D79110 Freiburg Germany
This book was carefully produced. Nevertheless, authors, editors and publisher do not warrant the information contained therein to be free of errors. Readers are advised to keep in mind that statements, data, illustrations, procedural details or other items may inadvertently be inaccurate.
Library of Congress Card No.: applied for. British Library CataloguinginPublication Data: A catalogue record for this book is available from the British Library. Die Deutsche Bibliothek — CIPCataloguinginPublication Data A catalogue record for this book is available from Die Deutsche Bibliothek. ISBN 3527302573
© WILEYVCH Verlag GmbH, Weinheim 2002 Printed on acidfree paper . All rights reserved (including those of translation into other languages). No part of this book may be reproduced in any form — by photoprinting, microfilm, or any other means — nor transmitted or translated into machine language without written permission from the publishers. Registered names, trademarks, etc. used in this book, even when not specifically marked as such, are not to be considered unprotected by law. Printing: Strauss Offsetdruck GmbH, Mörlenbach Bookbinding: Litges & Dopf Buchbinderei GmbH, Heppenheim Printed in the Federal Republik of Germany
Dedicated to Micheline Pﬁster, Sean and Nicolas Vogel, and in fond memory of Gerrit Jörgen Korvink
Maria Cristina Vecchi, Sarah Maria Greiner und im Gedenken an Gertrud Maria Greiner
Contents
Contents Preface Chapter 1 Introduction
7 13 15
The System Concept . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16 Popular Deﬁnitions and Acronyms . . . . . . . . . . . . . . . . . . 19 Semiconductors versus Conductors and Insulators . . . . . . . . 19 The Diode Family . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20 The Transistor Family . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20 Passive Devices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21 Microsystems: MEMS, MOEMS, NEMS, POEMS, etc. . . . . . 21
Sources of Information . . . . . . . . . . . . . . . . . . . . . . . . . . . 24 Summary for Chapter 1 . . . . . . . . . . . . . . . . . . . . . . . . . . . 24 References for Chapter 1 . . . . . . . . . . . . . . . . . . . . . . . . . 25
Semiconductors for Micro and Nanosystem Technology
7
Chapter 2 The Crystal Lattice System Observed Lattice Property Data
27
. . . . . . . . . . . . . . . . . . . . 29
Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33 Silicon Dioxide . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 36 Silicon Nitride . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 37 Gallium Arsenide . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 37
Crystal Structure
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 39
Symmetries of Crystals
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 40
Elastic Properties: The Stressed Uniform Lattice Statics
. . . . . . . 48
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48
The Vibrating Uniform Lattice
. . . . . . . . . . . . . . . . . . . . . 64
Normal Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 64 Phonons, Speciﬁc Heat, Thermal Expansion . . . . . . . . . . . . . 81
Modiﬁcations to the Uniform Bulk Lattice . . . . . . . . . . . . 88 Summary for Chapter 2 . . . . . . . . . . . . . . . . . . . . . . . . . . . 91 References for Chapter 2 . . . . . . . . . . . . . . . . . . . . . . . . . 92
Chapter 3 The Electronic System
95
Quantum Mechanics of Single Electrons
. . . . . . . . . . . . . 96
Wavefunctions and their Interpretation . . . . . . . . . . . . . . . . . 97 The Schrödinger Equation . . . . . . . . . . . . . . . . . . . . . . . . . . 102
Free and Bound Electrons, Dimensionality Effects
. . . . 106
Finite and Inﬁnite Potential Boxes . . . . . . . . . . . . . . . . . . . . 106 Continuous Spectra . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 Periodic Boundary Conditions . . . . . . . . . . . . . . . . . . . . . . . 115 Potential Barriers and Tunneling . . . . . . . . . . . . . . . . . . . . . 115 The Harmonic Oscillator . . . . . . . . . . . . . . . . . . . . . . . . . . . 118 The Hydrogen Atom . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123 Transitions Between Electronic States . . . . . . . . . . . . . . . . . 127 Fermion number operators and number states . . . . . . . . . . 130
Periodic Potentials in Crystal
. . . . . . . . . . . . . . . . . . . . . 132
The Bloch Functions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 132 Formation of Band Structure . . . . . . . . . . . . . . . . . . . . . . . . 133 Types of Band Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . 136 Effective Mass Approximation . . . . . . . . . . . . . . . . . . . . . . . 139
Summary for Chapter 3 . . . . . . . . . . . . . . . . . . . . . . . . . . 140 References for Chapter 3 . . . . . . . . . . . . . . . . . . . . . . . . 141
8
Semiconductors for Micro and Nanosystem Technology
Chapter 4 The Electromagnetic System 143 Basic Equations of Electrodynamics
. . . . . . . . . . . . . . . 144
TimeDependent Potentials . . . . . . . . . . . . . . . . . . . . . . . . .149 QuasiStatic and Static Electric and Magnetic Fields . . . . .151
Basic Description of Light
. . . . . . . . . . . . . . . . . . . . . . . 158
The Harmonic Electromagnetic Plane Wave . . . . . . . . . . . .158 The Electromagnetic Gaussian Wave Packet . . . . . . . . . . . .160 Light as Particles: Photons . . . . . . . . . . . . . . . . . . . . . . . . .162
Waveguides
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 164
Example: The Homogeneous Glass Fiber
. . . . . . . . . . . . . .166
Summary for Chapter 4 . . . . . . . . . . . . . . . . . . . . . . . . . . 167 References for Chapter 4 . . . . . . . . . . . . . . . . . . . . . . . . 168
Chapter 5 Statistics Systems and Ensembles
169 . . . . . . . . . . . . . . . . . . . . . . . . . 170
Microcanonical Ensemble . . . . . . . . . . . . . . . . . . . . . . . . . .171 Canonical Ensemble . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .174 Grand Canonical Ensemble . . . . . . . . . . . . . . . . . . . . . . . . .176
Particle Statistics: Counting Particles
. . . . . . . . . . . . . . . 178
MaxwellBoltzmann Statistics . . . . . . . . . . . . . . . . . . . . . . .178 BoseEinstein Statistics . . . . . . . . . . . . . . . . . . . . . . . . . . . .180 FermiDirac Statistics . . . . . . . . . . . . . . . . . . . . . . . . . . . . .181 Quasi Particles and Statistics . . . . . . . . . . . . . . . . . . . . . . . .182
Applications of the BoseEinstein Distributions . . . . . . . 183 Electron Distribution Functions . . . . . . . . . . . . . . . . . . . 184 Intrinsic Semiconductors Extrinsic Semiconductors
. . . . . . . . . . . . . . . . . . . . . . . . . . .184 . . . . . . . . . . . . . . . . . . . . . . . . . . .187
Summary for Chapter 5 . . . . . . . . . . . . . . . . . . . . . . . . . . 190 References for Chapter 5 . . . . . . . . . . . . . . . . . . . . . . . . 190
Chapter 6 Transport Theory The SemiClassical Boltzmann Transport Equation
191 . . . . 192
The Streaming Motion . . . . . . . . . . . . . . . . . . . . . . . . . . . . .193 The Scattering Term . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .195 The BTE for Phonons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .197 Balance Equations for Distribution Function Moments . . .197
Semiconductors for Micro and Nanosystem Technology
9
Relaxation Time Approximation
Local Equilibrium Description
. . . . . . . . . . . . . . . . . . . . . . 201
. . . . . . . . . . . . . . . . . . . . 204
Irreversible Fluxes and Thermodynamic Forces . . . . . . . . . 205 Formal Transport Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . 212 The Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 216
From Global Balance to Local NonEquilibrium
. . . . . . 219
Global Balance Equation Systems . . . . . . . . . . . . . . . . . . . . 220 Local Balance: The Hydrodynamic Equations . . . . . . . . . . 220 Solving the DriftDiffusion Equations . . . . . . . . . . . . . . . . . 222 Kinetic Theory and Methods for Solving the BTE . . . . . . . . 227
Summary for Chapter 6 . . . . . . . . . . . . . . . . . . . . . . . . . . 231 References for Chapter 6 . . . . . . . . . . . . . . . . . . . . . . . . 231
Chapter 7 Interacting Subsystems PhononPhonon
233
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 235
Phonon Lifetimes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 235 Heat Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 236
ElectronElectron
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 239
The Coulomb Potential (Poisson Equation) . . . . . . . . . . . . . 240 The Dielectric Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 Screening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 242 Plasma Oscillations and Plasmons . . . . . . . . . . . . . . . . . . . 243
ElectronPhonon
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 245
Acoustic Phonons and Deformation Potential Scattering . . 246 Optical Phonon Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . 249 Piezoelectricity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 251 Piezoelectric Transducers . . . . . . . . . . . . . . . . . . . . . . . . . . 258 Stress Induced Sensor Effects: Piezoresistivity . . . . . . . . . . 260 Thermoelectric Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 262
ElectronPhoton
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 267
Intra and Interband Effects . . . . . . . . . . . . . . . . . . . . . . . . . 268 Semiconductor Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 270
PhononPhoton
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 276
ElastoOptic Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 276 Light Propagation in Crystals: PhononPolaritons . . . . . . . 277
Inhomogeneities
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 279
Lattice Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 280 Scattering Near Interfaces (Surface Roughness, . . . . . . . . . 281
10
Semiconductors for Micro and Nanosystem Technology
Phonons at Surfaces . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .284 The PN Junction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .300 MetalSemiconductor Contacts . . . . . . . . . . . . . . . . . . . . . .313
Summary for Chapter 7 . . . . . . . . . . . . . . . . . . . . . . . . . . 324 References for Chapter 7 . . . . . . . . . . . . . . . . . . . . . . . . 324
Index
Semiconductors for Micro and Nanosystem Technology
327
11
Preface
This book addresses the engineering student and practising engineer. It takes an engineeringoriented look at semiconductors. Semiconductors are at the focal point of vast number of technologists, resulting in great engineering, amazing products and unheardof capital growth. The work horse here is of course silicon. Explaining how semiconductors like silicon behave, and how they can be manipulated to make microchips that work—this is the goal of our book. We believe that semiconductors can be explained consistently without resorting 100% to the complex language of the solid state physicist. Our approach is more like that of the systems engineer. We see the semiconductor as a set of welldeﬁned subsystems. In an approximately topdown manner, we add the necessary detail (but no more) to get to grips with each subsystem: The physical crystal lattice, and charge carriers in lattice like potentials. This elemental world is dominated by statistics, making strange observations understandable: This is the glue we need to put the systems together and the topic of a further chapter. Next we show the the
Semiconductors for Micro and Nanosystem Technology
13
ory needed to predict the behavior of devices made in silicon or other semiconducting materials, the building blocks of modern electronics. Our book wraps up the tour with a practical engineering note: We look at how the various subsystems interact to produce the observable behavior of the semiconductor. To enrich the subject matter, we tie up the theory with concise boxed topics interspersed in the text. There are many people to thank for their contributions, and for their help or support. To the Albert Ludwig University for creating a healthy research environment, and for granting one of us (Korvink) sabbatical leave. To Ritsumeikan University in Kusatsu, Japan, and especially to Prof. Dr. Osamu Tabata, who hosted one of us (Korvink) while on sabbatical and where one chapter of the book was written. To the ETH Zurich and especially to Prof. Dr. Henry Baltes, who hosted one of us (Korvink) while on sabbatical and where the book project was wrapped up. To Prof. Dr. Evgenii Rudnyi, Mr. Takamitsu Kakinaga, Ms. Nicole Kerness and Mr. Sadik Hafizovic for carefully reading through the text and ﬁnding many errors. To the anonymous reviewers for their invaluable input. To Ms. Anne Rottler for inimitable administrative support. To VCHWiley for their deadline tolerance, and especially to Dr. Jörn Ritterbusch and his team for support. To Micheline and Cristina for enduring our distracted glares at home as we fought the clock (the calendar) to ﬁnish, and for believing in us. Jan G. Korvink and Andreas Greiner, Freiburg im Breisgau, February 2002
14
Semiconductors for Micro and Nanosystem Technology
Chapter 1 Introduction
Semiconductors have complex properties, and in the early years of the twentieth century these were mainly discovered by physicists. Many of these properties have been harnessed, and have been exploited in ingenious microelectronic devices. Over the years the devices have been rendered manufacturable by engineers and technologists, and have spawned off both a multibillion € (or $, or ¥) international industry and a variety of other industrial minirevolutions including software, embedded systems, the internet and mobile communications. Semiconductors still lie at the heart of this revolution, and silicon has remained its champion, warding off the competitors by its sheer abundance, suitability for manufacturing, and of course its tremendous headstart in the ﬁeld. Silicon is the working material of an exciting, competitive world, presenting a seemingly endless potential for opportunities.
Chapter Goal The goal of this chapter is to introduce the reader to the ﬁeld of semiconductors, and to the purpose and organization of the book.
Semiconductors for Micro and Nanosystem Technology
15
Introduction
Chapter Roadmap
In this chapter we ﬁrst explain the conceptual framework of the book. Next, we provide some popular deﬁnitions that are in use in the ﬁeld. Lastly, we indicate some of the sources of information on new inventions.
1.1 The System Concept This book is about semiconductors. More precisely, it is about semiconductor properties and how to understand them in order to be exploited for the design and fabrication of a large variety of microsystems. Therefore, this book is a great deal about silicon as a paradigm for semiconductors. This of course implies that it is also about other semiconductor systems, namely for those cases where silicon fails to show the desired effects due to a lack of the necessary properties or structure. Nevertheless, we will not venture far away from the paradigmatic material silicon, with its overwhelming advantage for a wide ﬁeld of applications with low costs for fabrication. To quote the Baltes theorem [1.1]: To prove your idea, put in on silicon. Since you will need circuitry, make it with CMOS. If you want to make it useful, get it packaged. The more expensive fabrication becomes, the less attractive the material is for the design engineer. Designers must always keep in mind the cost and resources in energy and personnel that it takes to handle materials that need additional nonstandard technological treatment. This is not to say that semiconductors other than silicon are unimportant, and there are many beautiful applications. But most of today’s engineers encounter silicon CMOS as a process with which to realize their ideas for microscopic systems. Therefore, most of the emphasis of this book lies in the explanation of the properties and behavior of silicon, or better said, “the semiconductor system silicon”.
16
Semiconductors for Micro and Nanosystem Technology
The System Concept
A semiconductor can be viewed as consisting of many subsystems. For one, there are the individual atoms, combining to form a chunk of crystalline material, and thereby changing their behavior from individual systems to a composite system. The atomic length scale is still smaller than typical length scales that a designer will encounter, despite the fact that subnanometer features may be accessible through modern experimental techniques. The subsystems that this book discusses emerge when silicon atoms are assembled into a crystal with unique character. We mainly discuss three systems:
• the particles of quantized atom vibration, or phonons; • the particles of quantized electromagnetic radiation, or photons; • the particles of quantized charge, or electrons. There are many more, and the curious reader is encouraged to move on to other books, where they are treated more formally. The important feature of these subsystems is that they interact. Each interaction yields effects useful to the design engineer. Why do we emphasize the system concept this much? This has a lot to do with scale considerations. In studying nature, we always encounter scales of different order and in different domains. There are length scales that play a signiﬁcant role. Below the nanometer range we observe single crystal layers and might even resolve single atoms. Thus we become aware that the crystal is made of discrete constituents. Nevertheless, on a micrometer scale—which corresponds to several thousands of monatomic layers—the crystal appears to be a continuous medium. This means that at certain length scales a homogenous isotropic continuum description is sufﬁcient. Modern downsizing trends might force us to take at least anisotropy into account, which is due to crystal symmetry, if not the detailed structure of the crystal lattice including single defects. Nanotechnology changes all of this. Here we are ﬁnally designing at the atomic length scale, a dream that inspired the early twentieth century.
Semiconductors for Micro and Nanosystem Technology
17
Introduction
Almost everything becomes quantized, from thermal and electrical resistance to interactions such as the Hall effect. Time scale considerations are at least as important as length scales. They are governed by the major processes that take place within the materials. The shortest technological time scales are found in electronelectron scattering processes and are on the order of a few femtoseconds, followed by the interaction process of lattice vibrations and electronic systems with a duration of between a few hundreds of femtoseconds to a picosecond. Direct optical transitions from the conduction band to the valence band lie in the range of a few nanoseconds to a few microseconds. For applications in the MHz (106 Hz) and GHz (109 Hz) regime the details of the electronelectron scattering process are of minor interest and most scattering events may be considered to be instantaneous. For some quantum mechanical effects the temporal resolution of scattering is crucial, for example the intracollisional ﬁeld effect. The same considerations hold for the energy scale. Acoustic electron scattering may be considered elastic, that is to say, it doesn’t consume energy. This is true only if the system’s resolution lies well above the few meV of any scattering process. At room temperature ( 300 K) this is a good approximation, because the thermal energy is of the order of 25.4 meV. The level of the thermal energy implies a natural energy scale, at which the band gap energy of silicon of about 1.1 eV is rather large. For high energy radiation of several keV the band gap energy again is negligible. The above discussion points out the typical master property of a composite system: A system reveals a variety of behavior at different length (time, energy, …) scales. This book therefore demands caution to be able to account for the semiconductor as a system, and to explain its building blocks and their interactions in the light of scale considerations.
18
Semiconductors for Micro and Nanosystem Technology
Popular Definitions and Acronyms
1.2 Popular Deﬁnitions and Acronyms The microelectronic and microsystem world is replete with terminology and acronyms. The number of terms grows at a tremendous pace, without regard to aesthetics and grammar. Their use is ruled by expedience. Nevertheless, a small number have survived remarkably long. We list only a few of the most important, for those completely new to the ﬁeld.
1.2.1 Semiconductors versus Conductors and Insulators A semiconductor such as silicon provides the technologist with a very special opportunity. In its pure state, it is almost electrically insulating. Being in column IV of the periodic table, it is exceptionally balanced, and comfortably allows one to replace the one or other atom of its crystal with atoms from column III or V (which we will term P and N type doping). Doing so has a remarkable effect, for silicon then becomes conductive, and hence the name “semiconductor”. Three important features are easily controlled. The density of “impurity” atoms can vary to give a tremendously wide control over the conductivity (or resistance) of the bulk material. Secondly, we can decide whether electrons, with negative charge, or holes, with positive charge, are the dominant mechanism of current ﬂow, just by changing to an acceptor or donor atom, i.e., by choosing P or N type doping. Finally, we can “place” the conductive pockets in the upper surface of a silicon wafer, and with a suitable geometry, create entire electronic circuits. If silicon is exposed to a hot oxygen atmosphere, it forms amorphous silicon dioxide, which is a very good insulator. This is useful to make capacitor devices, with the SiO 2 as the dielectric material, to form the gate insulation for a transistor, and of course to protect the top surface of a chip. Silicon can also be grown as a doped amorphous ﬁlm. In this state we lose some of the special properties of semiconductors that we will explore in this book. In the amorphous form we almost have metallike Semiconductors for Micro and Nanosystem Technology
19
Introduction
behavior, and indeed, semiconductor foundries offer both real metals (aluminium, among others) and polysilicon as “metallic” layers.
1.2.2 The Diode Family The simplest device that one can make using both P and N doping is the diode. The diode is explained in Section 7.6.4. The diode is a oneway valve with two electrical terminals, and allows current to ﬂow through it in only one direction. The diode provides opportunities for many applications. It is used to contact metal wires to silicon substrates as a Shottkey diode. The diode can be made to emit light (LEDs). Diodes can detect electromagnetic radiation as photodetectors, and they form the basis of semiconductor lasers. Not all of these effects are possible using silicon, and why this is so is also explained later on.
1.2.3 The Transistor Family This is the true fame of silicon, for it is possible to make this versatile device in quantities unheard of elsewhere in the engineering world. Imagine selling a product with more than 10 9 working parts! Through CMOS (complimentary metal oxide semiconductor) it is possible to create reliable transistors that require extraordinary little power (but remember that very little times 10 9 can easily amount to a lot). The trend in miniaturization, a reduction in lateral dimensions, increase in operation speed, and reduction in power consumption, is unparalleled in engineering history. Top that up with a parallel manufacturing step that does not essentially depend on the number of working parts, and the stage is set for the revolution that we have witnessed. The transistor is useful as a switch inside the logic gates of digital chips such as the memories, processors and communications chips of modern computers. It is also an excellent ampliﬁer, and hence found everywhere where high quality analog circuitry is required. Other uses include magnetic sensing and chemical sensing.
20
Semiconductors for Micro and Nanosystem Technology
Popular Definitions and Acronyms
1.2.4 Passive Devices In combination with other materials, engineers have managed to miniaturize every possible discrete circuit component known, so that it is possible to create entire electronics using just one process: resistors, capacitors, inductors and interconnect wires, to name the most obvious. For electromagnetic radiation, waveguides, ﬁlters, interferometers and more have been constructed, and for light and other forms of energy or matter, an entirely new industry under the name of microsystems has emerged, which we now brieﬂy consider.
1.2.5 Microsystems: MEMS, MOEMS, NEMS, POEMS, etc. In North America, the acronym MEMS is used to refer to microelectromechanical systems, and what is being implied are the devices at the length scale of microelectronics that include some nonelectrical signal, and very often the devices feature mechanical moving parts and electrostatic actuation and detection mechanisms, and these mostly couple with some underlying electrical circuitry. A highly successful CMOS MEMS, produced by Inﬁneon Technologies, is shown in Figure 1.1. The device, a)
Figure 1.1. MEMS device. a) Inﬁneon’s surface micromachined capacitive pressure sensor with interdigitated signal conditioning Type KP120 for automotive BAP and MAP applications. b) SEM photograph of the pressure sensor cells compared with a human hair. Image © Inﬁneon Technologies, Munich [1.2].
b)
Semiconductors for Micro and Nanosystem Technology
21
Introduction
placed in a lowcost SMD package, is used in MAP and BAP tire pressure applications. With an annual production running to several millions, it is currently sold to leading automotive customers [1.2]. MEMS has to date spawned off two further terms that are of relevance to us, namely MOEMS, for microoptoelectromechanical systems, and NEMS, for the inevitable nanoelectromechanical systems. MOEMS can include entire miniaturized optical benches, but perhaps the most familiar example is the digital light modulator chip sold by Texas Instruments, and used in projection display devices, see Figure 1.2.
Figure 1.2. MOEMS device. This 30 µm by 30 µm device is a single pixel on a chip that has as many pixels as a modern computer screen display. Each mirror is individually addressable, and deﬂects light from a source to a systems of lenses that project the pixel onto a screen. Illustration © Texas Instruments Corp., Dallas [1.3].
As for NEMS, the acronym of course refers to the fact that a critical dimension is now no longer the large micrometer, but has become a factor 1000 smaller. The atomic force microscope cantilever [1.4] may appear to be a MEMSlike device, but since it resolves at the atomic diameter scale, it is a clear case of NEMS, see Figure 1.3. Another example is the distributed mirror cavity of solidstate lasers made by careful epitaxial growth of many different semiconductor layers, each layer a few nanometers thick. Of major commercial importance is the submicron microchip electronic device technology. Here the lateral size of a transistor gate is the key size, which we know has dropped to below 100
22
Semiconductors for Micro and Nanosystem Technology
Popular Definitions and Acronyms
Figure 1.3. NEMS devices. Depicted are two tips of an atomic force microscope, made in CMOS, and used to visualize the force ﬁeld surrounding individual atoms. Illustration © Physical Electronics Laboratory, ETH Zurich, Switzerland [1.4].
nm in university and industrial research laboratories. Among NEMS we count the quantum wire and the quantum dot, which have not yet made it to the technologicalcommercial arena, and of course any purposefullydesigned and functional molecular monolayer ﬁlm. POEMS, or polymer MEMS, are microstructures made of polymer materials, i.e., they completely depart from the traditional semiconductorbased devices. POEMS are usually made by stereo microlithography through a photopolymerization process, by embossing a polymer substrate, by milling and turning, and by injection moulding. This class of devices will become increasingly important because of their potentially low manufacturing cost, and the large base of materials available. In Japan, it is typical to refer to the whole ﬁeld of microsystems as Micromachines, and manufacturing technology as Micromachining. In Europe, the terms Microsystems, Microtechnology or Microsystem Technology have taken root, with the addition of Nanosystems and the inevitable Nanosystem Technology following closely. The European naming convention is popular since it is easily translated into any of a large number of languages (German: Mikrosystemtechnik, French: Microtechnique, Italian: tecnologia dei microsistemi, etc.).
Semiconductors for Micro and Nanosystem Technology
23
Introduction
1.3 Sources of Information We encourage every student to regularly consult the published literature, and in particular the following journals: IOP
• Journal of Micromechanics and Microengineering • Journal of Nanotechnology
IEEE
• Journal of Microelectromechanical Systems • Journal of Electron Devices • Journal of Sensors • Journal of Nanosystems
Other
• WileyVCH Sensors Update, a journal of review articles • MYU Journal of Sensors and Materials • Elsevier Journal of Sensors and Actuators • Springer Verlag Journal of Microsystem Technology • Physical Review • Journal of Applied Physics Of course there are more sources than the list above, but it is truly impossible to list everything relevant. Additional sources on the worldwideweb are blossoming (see e.g. [1.5]), as well as the emergence of standard texts on technology, applications and theory. A starting point is best taken from the lists of chapter references. Two useful textbook references are Sze’s book on the physics of semiconductor devices [1.6] and Middelhoek’s book on silicon sensors [1.7].
1.4 Summary for Chapter 1 Silicon is a very important technological material, and understanding its behavior is a key to participating in the largest industry ever created. To
24
Semiconductors for Micro and Nanosystem Technology
References for Chapter 1
understand the workings of the semiconductor silicon, it helps to approach it as a system of interacting subsystems. The subsystems comprise the crystal lattice and its quantized vibrations—the phonons, electromagnetic radiation and its quantized form— the photons, and the loosely bound quantized charges—the electrons. The interactions between these systems is a good model with which to understand most of the technologically useful behavior of silicon. To understand the ensuing topics, we require a background in particle statistics. To render the ideas useful for exploitation in devices such as diodes, transistors, sensors and actuators, we require an understanding of particle transport modelling. These topics are now considered in more detail in the six remaining chapters of the book.
1.5 References for Chapter 1 1.1 1.2 1.3 1.4
1.5 1.6 1.7
Prof. Dr. Henry Baltes, Private communication Prof. Dr. Christofer Hierold, Private communication. See e.g. http://www.dlp.com D. Lange, T. Akiyama, C. Hagleitner, A. Tonin, H. R. Hidber, P. Niedermann, U. Staufer, N. F. de Rooij, O. Brand, and H. Baltes, Parallel Scanning AFM with OnChip Circuitry in CMOS Technology, Proc. IEEE MEMS, Orlando, Florida (1999) 447452 See e.g. http://www.memsnet.org/ S. M. Sze, Physics of Semiconductor Devices, 2nd Ed., John Wiley and Sons, New York (1981) Simon Middelhoek and S. A. Audet, Silicon Sensors, Academic Press, London (1989)
Semiconductors for Micro and Nanosystem Technology
25
Chapter 2 The Crystal Lattice System
In this chapter we start our study of the semiconductor system with the crystals of silicon ( Si ) , adding some detail on crystalline silicon dioxide ( SiO 2 ) and to a lesser extent on gallium arsenide ( GaAs ) . All three are regular latticearrangements of atoms or atoms. For the semiconductors silicon and gallium arsenide, we will consider a model that completely decouple the behavior of the atoms from the valence electrons, assuming that electronic dynamics can be considered as a perturbation to the lattice dynamics, a topic dealt with in Chapter 3. For all the electrons of the ionic crystal silicon dioxide, as well as the bound electrons of the semiconductors, we here assume that they obediently follow the motion of the atoms. We will see that by applying the methods of classical, statistical and quantum mechanics to the lattice, we are able to predict a number of observable constitutive phenomena of interest—i.e., we are able to explain macroscopic measurements in terms of microscopic crystal lattice mechanics. The effects include an approximation for the elastic coef
Semiconductors for Micro and Nanosystem Technology
27
The Crystal Lattice System
ﬁcients of continuum theory, acoustic dispersion, speciﬁc heat, thermal expansion and heat conduction. In fact, going beyond our current goals, it is possible to similarly treat dielectric, piezoelectric and elastooptic effects. However, the predictions are of a qualitative nature in the majority of cases, mainly because the interatomic potential of covalently bonded atoms is so hard to come by. In fact, in a sense the potential is reverse engineered, that is, using measurements of the crystal, we ﬁt parameters that improve the quality of the models to make them in a sense “predictive”. Chapter Goal Our goal for this chapter is to explain the observed crystal data with preferably a single comprehensive model that accounts for all effects. Chapter Roadmap
Our road map is thus as follows. We start by stating some of the relevant observable data for the three materials Si , SiO 2 and GaAs , without more than a cursory explanation of the phenomena. Our next step is to get to grips with the concept of a crystal lattice and crystal structure. Beyond this point, we are able to consider the forces that hold together the static crystal. This gives us a method to describe the way the crystal responds, with stress, to a strain caused by stretching the lattice. Then we progress to vibrating crystal atoms, progressively reﬁning our method to add detail and show that phonons, or quantized acoustic pseudo “particles”, are the natural result of a dynamic crystal lattice. Considering the phonons in the lattice then leads us to a description of heat capacity. Moving away from basic assumptions, we consider the anharmonic crystal and ﬁnd a way to describe the thermal expansion. The section following presents a cursory look at what happens when the regular crystal lattice is locally deformed through the introduction of foreign atoms. Finally, we leave the inﬁnitelyextended crystal model and brieﬂy consider the crystal surface. This is important, because most microsystem devices are build on top of semiconductor wafers, and so are repeat
28
Semiconductors for Micro and Nanosystem Technology
Observed Lattice Property Data
edly subject to the special features and limitations that the surface introduces.
2.1 Observed Lattice Property Data Geometric Structure
The geometric structure of a regular crystal lattice is determined using xray crystallography techniques, by recording the diffraction patterns of xray photons that have passed through the crystal. From such a recorded pattern (see Figure 2.1 (a)), we are able to determine the reﬂection planes formed by the constituent atoms and so reconstruct the relative positions of the atoms. This data is needed to proceed with a geometric (or, strictly speaking, grouptheoretic) characterization of the crystal lattice’s symmetry properties. We may also use an atomic force microscope (AFM) to map out the force ﬁeld that is exerted by the constituent atoms on the surface of a crystal. From such contour plots we can reconstruct the crystal structure and determine the lattice constants. We must be careful, though, because we may observe special surface conﬁgurations in stead of the actual bulk crystal structure, see Figure 2.1 (b).
Elastic Properties
The relationship between stress and strain in the linear region is via the elastic property tensor, as we shall shortly derive in Section 2.3.1. To measure the elastic parameters that form the entries of the elastic property tensor, it is necessary to form special test samples of exact geometric shape that, upon mechanical loading, expose the relation between stress and strain in such a way that the elastic coefﬁcients can be deduced from the measurement. The correct choice of geometry relies on the knowledge of the crystal’s structure, and hence its symmetries, as we shall see in Section 2.2.1. The most common way to extract the mechanical properties of crystalline materials is to measure the directiondependent velocity of sound inside the crystal, and by diffracting xrays through the crystal (for example by using a synchrotron radiation source).
Semiconductors for Micro and Nanosystem Technology
29
The Crystal Lattice System
(a)
(b)
Figure 2.1. (a) The structure of a silicon crystal as mapped out by xray crystallography in a Laue diagram. (b) The famous 〈 111〉 7 × 7 reconstructed surface of silicon as mapped out by an atomic force microscope. The bright dots are the Adatoms that screen the underlying lattice. Also see Figure 2.30.
Dispersion Curves
Dispersion curves are usually measured by scattering a neutron beam (or xrays) in the crystal and measuring the directiondependent energy lost or gained by the neutrons. The absorption or loss of energy to the crystal is in the form of phonons.
Thermal Expansion
Thermal expansion measurements proceed as for the stressstrain measurement described above. A thermal strain is produced by heating the sample to a uniform temperature. Armed with the knowledge of the elastic parameters, the inﬂuence of the thermal strain on the velocity of sound may then be determined. The material data presented in the following sections and in Table 2.1 was collected from references [2.5, 2.6]. Both have very complete tables of measured material data, together with reference to the publications where the data was found.
30
Semiconductors for Micro and Nanosystem Technology
Crystalline Silicon Semiconductors for Micro and Nanosystem Technology
Property
Si
LPCVD PolySi
Atomic Weight
Si: 28.0855
Si: 28.0855 .
Process
Gallium Arsenide
α Quartz
Si 3 N 4
GaAs
Si: 28.0855
Si: 28.0855
Si: 28.0855
O: 15.994
O: 15.994
N: 14.0067
Ga: 69.72 As: 74.9216
Thermal Oxide SiO 2
Carbonlike, Cubic symmetry
Polycrystalline
Amorphous
Trigonal symmetry
Amorphous
Zincblende Cubic symmetry
Density ( kg ⁄ m )
2330
2330
< 2200
2650
3100
5320
Elastic moduli ( Gpa ) Y: Young modulus B: Biaxial modulus S: Shear modulus C i : Tensor
Pure: C 11 : 166
Y: 130 – 174 S: 69
Y: 72 – 75
Y: 87
Y: 97 – 320 B: 249  311
Pure: C 11 : 118.1
Crystal class/ Symmetry 3
coefﬁcients.
C 12 : 63.9
C 12 : 53.2
C 44 : 79.6
C 44 : 59.4
pType: C 11 : 80.5 C 12 : 115 C 44 : 52.8
nType: C 11 : 97.1 C 12 : 54.8 C 44 : 172
Observed Lattice Property Data
Table 2.1. Lattice properties of the most important microsystem base materialsa.
31
Crystalline Silicon Property Semiconductors for Micro and Nanosystem Technology
Hardness ( Gpa )
Process
Gallium Arsenide
α Quartz
Si 3 N 4
GaAs
14.4 – 18
8.2


5.43 , polycrystal
Amorphous
X i 4.9127
Amorphous
5.65
Si
LPCVD PolySi
Thermal Oxide SiO 2
〈 100〉 :
10.5 – 12.5
5.1 – 13 ; 〈 111〉 : 11.7
Lattice parameter ( ) X, C: axes
5.43
Melting point ( °C )
1412
1412 .
1705

1902

Poisson ratio ν˜
〈 100〉 : 0.28
0.2 – 0.3
0.17  0.22
0.169
0.26
0.31
C 5.4046
〈 111〉 : 0.36
Speciﬁc heat C p ( J ⁄ kgK
702.24
702.24
740
740
750
350
Thermal conductivity ( W ⁄ mK )
150
150
1.1  1.5
1.4
18
46 ( 12 )
XY cut 14.3 Z cut 7.8
2.7 ×10
Thermal expansion coefﬁcient α (T
–1
)
–6
2.33 ×10
–6
2.33 ×10
–6
0.4 ×10
–6
0.55 ×10

a. The tabulated values for amorphous process materials are foundrydependent and are provided only as an indication of typical values. Also, many of the measurements on crystalline materials are for doped samples and hence should be used with care. Properties depend on the state of the material, and a common choice is to describe them based on the temperature and the pressure during the measurements. For technological work, we require the properties under operating conditions, i.e., at room temperature and at 1 atmosphere of pressure.
–6
–6
6.86 ×10
The Crystal Lattice System
32
Table 2.1. Lattice properties of the most important microsystem base materialsa.
Observed Lattice Property Data
2.1.1 Silicon A semiconductor quality Silicon ingot is a gray, glassy, facecentered crystal. The element is found in column IV of the periodic table. It has the same crystal structure as diamond, as illustrated in Figure 2.2. Silicon
(a)
(b)
(c)
(d)
(e)
Figure 2.2. The diamondlike structure of the Silicon crystal is caused by the tetrahedral 3 arrangement of the four sp bondforming orbitals of the silicon atom, symbolically shown (a) as stippled lines connecting the balllike atomic nuclei in this tetrahedral repeating unit. (b) When the atoms combine to form a crystal, we observe a structure that may be viewed as a set of two nested cubic lattices, or (c) a single facecentered cubic lat3 tice with a basis. (d) The structure of the sp hybrid bonds. (e) The fcc unit cell can also be viewed as four tetrahedra.
has a temperature dependent coefﬁcient of thermal expansion in K described by Semiconductors for Micro and Nanosystem Technology
–1
33
The Crystal Lattice System
α(T ) –3
–4
= ( 3.725 ( 1 – exp ( – 5.88 ×10 ( T – 124 ) ) ) + 5.548 ×10 T ) ×10 and a lattice parameter (the interatomic distance in temperature as
–6
) that varies with
a(T ) –5
–9
(2.1)
= 5.4304 + 1.8138 ×10 ( T – 298.15 ) + 1.542 ×10 ( T – 298.15 )
2
(2.2)
We will later take a more detailed look at the thermal strain ε ( T – T 0 ) = α ( T ) ( T – T 0 ) . Both α ( T ) and a ( T ) are plotted in Figure 2.3. Both of 5.440
4 ×10
–6
5.438 2 ×10
5.436 5.434
400
–6
800 0
Temperature in K
0
600 1200 Temperature in K
Figure 2.3. The thermal expansion properties of Silicon. Shown on the left is the temperature dependence of the lattice parameter (the size of a unit cell), and to its right is the temperature dependence of the thermal expansion coefﬁcient. The typical engineering temperature range for silicon electronic devices is indicated by the background gray boxes.
these properties are also dependent on the pressure experienced by the material, hence we should write α ( T , p ) and a ( T , p ) . It is important to note that “technological” silicon is doped with foreign atoms, and will in general have material properties that differ from the values quoted in Table 2.1, but see [2.6] and the references therein. Silicon’s phonon dispersion diagram is shown in Figure 2.4.
34
Semiconductors for Micro and Nanosystem Technology
Observed Lattice Property Data
ω(k )
X U
W K
Γ L
k Γ
∆
X U, K Σ
Γ
Λ
k L L
K
W
X
Figure 2.4. The measured and computed dispersion diagrams of crystalline silicon. The vertical axis represents the phonon frequency, the horizontal axis represents straightline segments in kspace between the main symmetry points of the Brillouin zone, which is shown as an insert. Figure adapted from [2.5].
Silicon is the carrier material for most of today’s electronic chips and microsystem (or microelectromechanical system (MEMS), or micromachine) devices. The ingot is sliced into wafers, typically 0.5 mm thick and 50 to 300 mm in diameter. Most electronic devices are manufactured in the ﬁrst 10 µ m of the wafer surface. MEMS devices can extend all the way through the wafer. Cleanroom processing will introduce foreign dopant atoms into the silicon so as to render it more conducting. Other processes include subtractive etching steps, additive deposition steps and modiﬁcations such as oxidation of the upper layer of silicon. Apart from certain carefully chosen metal conductors, the most common materials used in conjunction with silicon are ovengrown or deposited thermal silicon oxides and nitrides (see the following sections), as well as polycrystalline silicon.
Semiconductors for Micro and Nanosystem Technology
35
The Crystal Lattice System
IC process quality LPCVD polycrystalline silicon (PolySi) has properties that depend strongly on the foundry of origin. It is assumed to be isotropic in the plane of the wafer, and is mainly used as a thin ﬁlm thermal and electrical conductor for electronic applications, and as a structural and electrode material for MEMS devices.
2.1.2 Silicon Dioxide Crystalline silicon dioxide is better known as fused quartz. It is unusual to obtain quartz from a siliconbased process, say CMOS, because the production of crystalline quartz usually requires very high temperatures that would otherwise destroy the carefully produced doping proﬁles in the silicon. Semiconductorrelated silicon dioxide is therefore typically amorphous. Since quartz has a noncubic crystal structure, and therefore displays useful properties that are not found in highsymmetry cubic systems such as silicon, yet are of importance to microsystems, we also include it in our discussion. We consider α quartz, one of the variants of quartz that is
Figure 2.5. Three perspective views of the trigonal unit cell of α Quartz. From left to right the views are towards the origin along the X 1 , X 2 and the C axes. The six large spheres each with two bonds represent oxygen atoms, the three smaller spheres each with four tetrahedral bonds represent silicon atoms.
36
Semiconductors for Micro and Nanosystem Technology
Observed Lattice Property Data o
stable below 573 C , with trigonal crystal symmetry. The unit cell of the quartz crystal is formed by two axes, called X 1 and X 2 , at 60° to each other, see Figure 2.5. Quartz is noncentrosymmetric and hence piezoelectric. It also has a handedness as shown in Figure 2.6.
Figure 2.6. α Quartz is found as either a right or a lefthanded structure, as indicated by the thick lines in the structure diagram that form a screw through the crystal. In the ﬁgure, 8 unit cells are arranged in a ( 2 × 2 × 2 ) block.
2.1.3 Silicon Nitride Crystalline silicon nitride (correctly known as trisilicon tetranitride) is not found on silicon IC wafers because, as for silicon dioxide, very high temperatures are required to form the pure crystalline state, see Figure 2.7. These temperature are not compatible with silicon foundry processing. In fact, on silicon wafers, silicon nitride is usually found as an amorphous mixture that only approaches the stochiometric relation of Si 3 N 4 , the speciﬁc relation being a strong function of process parameters and hence is ICfoundry speciﬁc. In the industry, it is variously referred to as “nitride”, “glass” or “passivation”, and may also contain amounts of oxygen.
2.1.4 Gallium Arsenide Crystalline gallium arsenide (GaAs) is a “goldgray” glassy material with the zincblende structure. When bound to each other, both gallium and arsenic atoms form tetrahedral bonds. In the industry, GaAs is referred to as a IIIV (threeﬁve), to indicate that it is a compound semiconductor Semiconductors for Micro and Nanosystem Technology
37
The Crystal Lattice System
Figure 2.7. Silicon nitride appears in many crystalline conﬁgurations. The structure of α and of β Si 3 N 4 are based on vertical stacks of SiN 4 tetrahedra, as shown in (I) and (II) respectively.
(I)
(II)
whose constituents are taken from the columns III and V of the periodic table. The atoms form into a zincblende crystal, structurally similar to the diamondlike structure of silicon, but with gallium and arsenic atoms alternating, see Figure 2.8.
Figure 2.8. The zincblende structure of gallium arsenide. The two atom types are represented by spheres of differing diameter. Also see Figure 2.2.
38
Semiconductors for Micro and Nanosystem Technology
Crystal Structure
Gallium arsenide is mainly used to make devices and circuits for the allimportant optoelectronics industry, where its raw electronic speed or the ability to act as an optoelectronic lasing device is exploited. It is not nearly as popular as silicon, though, mainly because of the prohibitive processing costs. Gallium arsenide has a number of material features that differ signiﬁcantly from Silicon, and hence a reason why we have included it in our discussion here. Gallium arsenide’s phonon dispersion diagram is shown in Figure 2.9. ω(k )
W K
X U Γ L
k Γ
∆
X
X U, K
Σ
Γ
Λ
L
Figure 2.9. The measured and computed dispersion diagrams of crystalline gallium arsenide. The vertical axis represents the phonon frequency, the horizontal axis represents straightline segments in kspace between the main symmetry points of the Brillouin zone, which is shown as an insert. Figure adapted from [2.5].
2.2 Crystal Structure As we have seen, crystals are highly organized regular arrangements of atoms or ions. They differ from amorphous materials, which show no regular lattice, and polycrystalline materials, which are made up of adjacent irregularlyshaped crystal grains, each with random crystal orienta
Semiconductors for Micro and Nanosystem Technology
39
The Crystal Lattice System
tion. From observations and measurements we ﬁnd that it is the regular crystalline structure that leads to certain special properties and behavior of the associated materials. In this section we develop the basic ideas that enable us to describe crystal structure analytically, so as to exploit the symmetry properties of the crystal in a systematic way.
2.2.1 Symmetries of Crystals Consider a regular rectangular arrangement of points on the plane. The points could represent the positions of the atoms that make up a hypothetical twodimensional crystal lattice. At ﬁrst we assume that the atoms are equally spaced in each of the two perpendicular directions, say by a pitch of a and b . More general arrangements of lattice points are the rule. Translational Invariance
Consider a vector a that lies parallel to the horizontal lattice direction and with magnitude equal to the pitch a . Similarly, consider vector b in the other lattice direction with magnitude equal to the pitch b . Then, starting at point p i , we can reach any other lattice point q j with q j = α j a + β j b , where α j and β j are integers. Having reached another interior point q j , the vicinity is the same as for point p i , and hence we say that the lattice is invariant to translations of the form α j a + β j b , see the example in Figure 2.10.
Figure 2.10. In this 2dimensional inﬁnitelyextending regular lattice the 2 lattice vectors are neither perpendicular nor of equal length. Given a starting point, all lattice points can be reached through q j = α j a + β j b . The vicinities of p i and q i are similar.
40
q j = 2a + 5b qj
pi
b a
Semiconductors for Micro and Nanosystem Technology
b
a
Crystal Structure
Rotational Symmetry
If we consider the vicinity of an interior point p i in our lattice, and let us assume that we have very many points in the lattice, we see that by rotating the lattice in the plane about point p i by an angle of 180° , the vicinity of the point p i remains unchanged. We say that the lattice is invariant to rotations of 180° . Clearly, setting a = b and a ⊥ b makes the lattice invariant to rotations of 90° as well. Rotational symmetry in lattices are due to rotations that are multiples of either 60° , 90° or 180° , see Figure 2.11. If the underlying lattice has a rotational symmetry, we will expect the crystal’s material properties to have the same symmetries.
180°
90°
60°
Figure 2.11. Illustrations of lattice symmetries w.r.t. rotations.
Bravais Lattice
With the basic idea of a lattice established, we now use the concept of a Bravais lattice to model the symmetry properties of a crystal’s structure. A Bravais lattice is an inﬁnitely extending regular threedimensional array of points that can be constructed with the parametrized vector q j = α ja + β jb + γ jc
(2.3)
where a , b and c are the noncoplanar lattice vectors and α j , β j and γ j are arbitrary (positive and negative) integers. Note that we do not Semiconductors for Micro and Nanosystem Technology
41
The Crystal Lattice System
assume that the vectors a , b and c are perpendicular. The Bravais lattice is inherently symmetric with respect to translations q j : this is the way we construct it. The remainder of the symmetries are related to rotations and reﬂections. There are 7 crystal systems: hexagonal, trigonal, triclinic, monoclinic, orthorhombic, tetragonal and cubic. In addition, there are 14 Bravais lattice types, see Figure 2.12. These are grouped into the following six lattice systems in decreasing order of geometric generality (or increasing order of symmetry): triclinic, monoclinic, orthorhombic, tetragonal, Hexagonal and cubic. The facecentered cubic (fcc) diamondlike lattice structure of silicon is described by the symmetric arrangement of vectors shown in Figure 2.13 (I). The fcc lattice is symmetric w.r.t. 90o rotations about all three coordinate axes. Gallium arsenide´s zincblende bccstructure is similarly described as for silicon. Because of the presence of two constituent atoms, GaAs does not allow the same translational symmetries as Si. Primitive Unit Cell
We associate with a lattice one or more primitive unit cells. A primitive unit cell is a geometric shape that, for singleatom crystals, effectively contains one lattice point. If the lattice point is not in the interior of the primitive cell, then more than one lattice point will lie on the boundary of the primitive cell. If, for the purpose of illustration, we associate a sphere with the lattice point, then those parts of the spheres that overlap with the inside of the primitive cell will all add up to the volume of a single sphere, and hence we say that a single lattice point is enclosed. Primitive cells seamlessly tile the space that the lattice occupies, see Figure 2.14.
WignerSeitz Unit Cell
The most important of the possible primitive cells is the WignerSeitz cell. It has the merit that it contains all the symmetries of the underlying Bravais lattice. Its deﬁnition is straightforward: The WignerSeitz cell of lattice point p i contains all spatial points that are closer to p i than to any other lattice point q j . Its construction is also straightforward: Considering lattice point p i , connect p i with its neighbor lattice points q j . On each connection line, construct a plane perpendicular to the connecting line at a position halfway along the line. The planes intersect each other
42
Semiconductors for Micro and Nanosystem Technology
Crystal Structure
TC
OP
T
OI
MI
MP
OC
OF
HP
HR
TI TP
CF CI CP Figure 2.12. The fourteen Bravais lattice types. CP: Cubic P; CI: Bodycentered cubic; CF: Facecentered cubic; a = b = c , α = β = γ = 90° . TP: Tetragonal; TI: Bodycentered tetragonal; a = b ≠ c , α = β = γ = 90° . HP: Hexagonal; HR: Hexagonal R; a = b ≠ c , α = β = 90° , γ = 120° (this not a separate Bravais lattice type). OP: Orthorhombic; OI: Bodycentered orthorhombic; OF: Facecentered orthorhombic; OC: Corthorhombic; a ≠ b ≠ c , α = β = γ = 90° . MP: Monoclinic; MI: Facecentered monoclinic; a ≠ b ≠ c , α = β = 90° ≠ γ . T: Trigonal; a = b = c , α ≠ β ≠ γ . TC: Triclinic; a ≠ b ≠ c , α ≠ β ≠ γ . a, b, c refer to lattice pitches; α, β, γ to lattice vector angles.
Semiconductors for Micro and Nanosystem Technology
43
The Crystal Lattice System
b b
c
c
a
a Figure 2.13. The equivalent lattice vectors sets that deﬁne the structures of the diamondlike fcc structure of Si and the zincblendelike structure of GaAs . The vectors are either the set: a = ( 2, 0, 0 ) , b = ( 0, 2, 0 ) , c = ( 0.5, 0.5, 0.5 ) or the set: a = ( 0.5, 0.5, – 0.5 ) , b = ( 0.5, – 0.5, 0.5 ) , c = ( 0.5, 0.5, 0.5 ) .
Figure 2.14. Illustrations of some of the many primitive unit cells for a 2dimensional lattice. Of these, only (g) is a WignerSeitz cell. Figure adapted from [2.10].
(f) (e)
(c) (b) (a)
(g)
(d)
and, taken together, deﬁne a closed volume around the lattice point p i . The smallest of these volumes is the WignerSeitz cell, illustrated in Figure 2.15. Reciprocal Lattice
The spatial Bravais crystal lattice is often called the direct lattice, to refer to the fact that we can associate a reciprocal lattice with it. In fact, in studying the properties of the crystal lattice, most data will be referred to
44
Semiconductors for Micro and Nanosystem Technology
Crystal Structure
(I)
(II) (III)
Figure 2.15. The WignerSeitz cell for the bcc lattice. (I) shows the cell without the atomic positions. (II) includes the atomic positions so as to facilitate understanding the method of construction. (III) The WignerSeitz cell tiles the space completely.
the reciprocal lattice. Let us consider a plane wave (see Box 2.1), traversing the lattice, of the form e
ik • r
.
(2.4)
We notice two features of this expression: the vectors k and r are symmetrical in the expression (we can swap their positions without altering the expression); and the crystal is periodic in r space. The vector r is a position in real space; the vector k is called the position vector in reciprocal space, and often also called the wave vector, since it is “deﬁned” using a plane wave. Next, we consider waves that have the same periodicity as the Bravais lattice. The Bravais lattice points lie on the regular grid described by the vectors q , so that a periodic match in wave amplitude is expected if we move from one grid position to another, and therefore e
ik • ( r + q )
= e
ik • r
.
(2.5)
This provides us with a condition for the wave vector k for waves that have the same spatial period as the atomic lattice, because we can cancel ik • r out the common factor e to obtain e
ik • q
0
= 1 = e .
Semiconductors for Micro and Nanosystem Technology
(2.6)
45
The Crystal Lattice System
Equation (2.6) generates the k (wave) vectors from the q (lattice position) vectors, and we see that these are mutually orthogonal. We summarize the classical results of the reciprocal lattice: Reciprocal Lattice Properties
• The reciprocal lattice is also a Bravais lattice. • Just as the direct lattice positions are generated with the primitive unit vectors q j = α j a + β j b + γ j c , the reciprocal lattice can also be so generated using k j = δ j d + ε j e + ζ j f . The relation between the two primitive vector sets is b×c d = 2π a ⋅ (b × c)
(2.7a)
c×a e = 2π a ⋅ (b × c)
(2.7b)
a×b f = 2π a ⋅ (b × c)
(2.7c)
• The reciprocal of the reciprocal lattice is the direct lattice. • The reciprocal lattice also has a primitive cell. This cell is called the Brillouin zone after its inventor.
• The volume of the direct lattice primitive cell is v = a ⋅ ( b × c ) . • The
volume of the reciprocal lattice V = d ⋅ ( e × f ) . From (2.7c) we see that 2π d =  ( b × c ) v
2π e =  ( c × a ) v
primitive
2π f =  ( a × b ) v
cell
is
(2.8)
and hence that 3
( 2π ) V = v
(2.9)
Miller Indices The planes formed by the lattice are identiﬁed using Miller indices. These are deﬁned on the reciprocal lattice, and are deﬁned as the coordinates of the shortest reciprocal lattice vector that is normal to the plane. Thus, if we consider a plane passing through the crystal, the Miller indi
46
Semiconductors for Micro and Nanosystem Technology
Crystal Structure
Box 2.1. Plane waves and wavevectors. We describe a general plane wave with i ( k ⋅ r – ωt )
ψ ( r, t ) = Ae . (B 2.1.1) Recalling the relation between the trigonometric functions and the exponential function, iθ
(B 2.1.2) e = cos ( θ ) + i sin ( θ ) . we see that ψ is indeed a wavelike function, for θ parametrizes an endless circular cycle on the complex plane. I
e
θ
iθ
counts the number cycles completed along a spatial segment. If we ﬁx the time t (“freezing” the wave in space and time), then moving along a spatial direction we will experience a wavelike variation of the amplitude of ψ as k ⋅ r . If we now move in a direction perpendicular to the propagation of the wave k , then we will experience no amplitude modulation. Next, staying in the perpendicular direction to the wave propagation at a ﬁxed position, if the time is again allowed to vary, we will now experience an amplitude modulation as the wave moves past us.
R
Figure B2.1.1: The exponential function describes a cycle in the complex plane. Equation (B 2.1.1) is a powerful way of describing a plane wave. Two vectors, the spatial position vector r and the wave vector, or reciprocal position vector k , are position arguments to the exponential function. The cyclic angle that it the wave has rotated through is the complete factor ( k ⋅ r – ωt ) . Since r measures the distance along an arbitrary spatial direction and k points along the propagation direction of the wave, k ⋅ r gives the component of this parametric angle. k measures rotation angle per distance travelled (a full cycle of 2π is one wavelength), so that k ⋅ r
x
t
Figure B2.1.2: The appearance of a 1dimensional wave plotted for t and x as parameters. If t is kept stationary, moving in the xdirection is accompanied by a wavelike variation.
ces are the components of a k space vector (the vector is normal to the plane) that fulﬁl k ⋅ r = Constant , where r lies on the plane of interest. As an example, consider a cubic lattice with the Miller indices ( m, n, p ) of a plane that lies parallel to a face of the cube. The indices determine the planenormal k space vector k = mb 1 + nb 2 + pb 3 . The plane is Semiconductors for Micro and Nanosystem Technology
47
The Crystal Lattice System
k ⋅ r = Constant = 2π ( r 1 m + r 2 n + r 3 p ) . ﬁxed by Since k ⋅ a 1 = 2πm , k ⋅ a 2 = 2πn and k ⋅ a 3 = 2πp , the space axis interr 1 = Constant ⁄ 2πm , cepts for the plane are therefore r 2 = Constant ⁄ 2πn and r 3 = Constant ⁄ 2πp . Silicon Reciprocal Lattice Shape
We have seen that the silicon crystal can be represented by a facecentered cubic lattice with a basis. This means that its reciprocal lattice is a bodycentered lattice with a basis. This has the following implications. The WignerSeitz cell for the silicon direct lattice is a rhombic dodecahedron, whereas the ﬁrst Brillouin zone (the WignerSeitz cell of the reciprocal lattice) is a truncated dodecahedron.
2.3 Elastic Properties: The Stressed Uniform Lattice In a broad sense the geometry of a crystal’s interatomic bonds represent the “structural girders” of the crystal lattice along which the forces act that keep the crystal intact. The strength of these directional interatomic forces, and the way in which they respond to small geometrical perturbations; these are the keys that give a crystal lattice its tensorial elastic properties and that enable us to numerically relate applied stress to a strain response. In this section we derive the Hooke law for crystalline, amorphous and polycrystalline materials based on lattice considerations.
2.3.1 Statics Atomic Bond Model
It is well known that atoms form different types of bonds with each other. The classiﬁcation is conveniently viewed as the interaction between a pair of atoms:
• Ionic—a “saturated” bond type that is characterized by the fact that one atom ties up the electrons participating in the bond in its outermost shell. This leaves the two atoms oppositely charged. The cou
48
Semiconductors for Micro and Nanosystem Technology
Elastic Properties: The Stressed Uniform Lattice
lombic (electrostatic) force between the net charges of the constituent “ions” form the bond. This bond is sometimes termed localized, because the electrons are tightly bound to the participating atoms.
• van der Waals—a very weak bonding force that is often termed the ﬂuctuating dipole force because it is proportional to an induced dipole between the constituent atoms, and this effective dipole moment has a nonvanishing time average.
• Valency—another localized electronpair bond. Here, the electronpair of the participating atoms form a hybrid orbital that is equally shared by the two atoms, hence the term covalent. Clearly, ionic and covalent bonds are the two limiting cases of a similar phenomena, so that a bond inbetween these limits can also be expected. Valency bonds are quite strong, and account for the hardness and brittle nature of the materials.
• Metallic—the electrons participating in the bonding are nonlocalized. Typically, the number of valence electrons at a point is exceeded by the number of nearestneighbor atoms. The electrons are therefore shared by many atoms, making them much more mobile, and also accounts for the ductility of the material. a)
b)
1 σ 1 =  ( s + p x + p y + p z ) 2 1 σ 3 =  ( s – p x + p y – p z ) 2
c)
1 σ 2 =  ( s + p x – p y – p z ) 2 1 σ 4 =  ( s – p x – p y + p z ) 2
Figure 2.16. The geometry of a tetrahedral bond for Carbonlike atoms can be repre3 sented by a hybrid sp function as a superposition of 2s and 2porbitals. a) sorbital. b) 3 porbital. c) s p orbital. Semiconductors for Micro and Nanosystem Technology
49
The Crystal Lattice System
The semiconductors that we consider are covalently bonded. We now give a qualitative description of the tetrahedral covalent bond of the atoms of an fcc crystal. Solving the Schrödinger equation (see Box 2.2 Box 2.2. The stationary Schrödinger equation and the Hamiltonian of a Solid [2.4]. In principle, all basic calculations of solid state properties are computed with the Schrödinger equation Hϕ = Eϕ (B 2.2.1) The Hamiltonian operator H deﬁnes the dynamics and statics of the model, ϕ represents a state of the model, and E is the scalarvalued energy. Thus the Schrödinger equation is an Eigensystem equations with the energy plying the role of an eigenvalue and the state the role of an eigenfunction. The Hamiltonian is usually built up of contributions from identiﬁable subcomponents of the system. Thus, for a solidstate material we write that H = H e + H i + H ei + H x
(B 2.2.2)
i.e., the sum of the contributions from the electrons, the atoms, their interaction and interactions with external inﬂuences (e.g., a magnetic ﬁeld). Recall that the Hamiltonian is the sum of kinetic and potential energy terms. Thus, for the electrons we have H e = T e + U ee 2
=
pα
1
e
2
+  ′ ∑ 2m 8πε 0 ∑ r α – r β α
The second term is the Coulombic potential energy due to the electron charges. Note that the sum is primed: the sum excludes terms where α = β. For the atoms the Hamiltonian looks similar to that of the electron H i = T i + U ii 2
=
Pα
1
+  ′V ( R – R β ) ∑ 2M 2 ∑ i α α
(B 2.2.4)
αβ
For the electronatom interaction we associate only a potential energy H ei = U ei =
∑ V ei ( rα – Rβ )
(B 2.2.5)
αβ
Equation (B 2.2.1) is hardly ever solved in all its generality. The judicious use of approximations and simpliﬁcations have yielded not only tremendous insight into the inner workings of solid state materials, but have also been tremendously successful in predicting complex phenomena. We will return to this topic in the next chapter, where we will calculate the valence band structure of silicon to remarkable accuracy.
(B 2.2.3)
αβ
and Chapter 3) for a single atom yields the orthogonal eigenfunctions that correspond to the energy levels of the atom, also known as the orbitals. The spherical harmonic functions shown in Table 2.2 are such eigenfunctions. The tetrahedral bond structure of the Si atom can be made, 3 through a superposition of basis orbitals, to form the hybrid s p orbital
50
Semiconductors for Micro and Nanosystem Technology
Elastic Properties: The Stressed Uniform Lattice
m
2
Table 2.2. The spherical harmonic functions Y l ( θ, φ ) , Also see Table 3.1 and Figure 3.9 in Chapter 3. l
m Plot
l
m Plot
0
0
1
l
m Plot
0
1
1
2
0
2
3
0
4
0
l
m Plot
1
2
2
3
1
3
2
3
3
4
1
4
2
4
3
that we associate with its valence electrons. The construction is illustrated in Figure 2.16. The valence electron orbitals may overlap to form bonds between atoms. The interpretation is straightforward: a valence electron’s orbital represents the probability distribution of ﬁnding that electron in a speciﬁc region of space. In a ﬁrst approximation, we let the orbitals simply overlap and allow them to interfere to form a new shared orbital. Bonding takes place if the new conﬁguration has a lower energy than the two separate atom orbitals. The new, shared, hybrid orbital gives the electrons of
Semiconductors for Micro and Nanosystem Technology
51
The Crystal Lattice System
the two binding atoms a relatively high probability of occupying the space between the atoms. Figure 2.17 shows what happens when atoms bond to form a diamond
a
a
E(r) r
a
(I)
(II)
r=a
Figure 2.17. When atoms with a tetrahedral bond structure form a covalentlybonded crystal lattice, the valence electrons are localized about the nearestneighbor atoms. We visualize these (I) as the overlap positions of the sp3hybrid orbitals, shown here for four atoms in a diamondlike lattice. We assume that the distance a between the atomic cores, the lattice constant, is the position of minimum energy for the bond (II).
like crystal. The energy of the atomic arrangement is lowered to a minimum when all atoms lie approximately at a separation equal to the lattice constant a (the lattice constant is the equilibrium distance that separates 3 atoms of a lattice). The s p orbitals of neighboring atoms overlap to form new shared orbitals. The electrons associated with these new states are effectively shared by the neighboring atoms, but localized in the bond. The bonding process does not alter the orbitals of the other electrons signiﬁcantly. The potential energy plot of Figure 2.17 (II) is necessarily only approximate, yet contains the necessary features for a single ionic bond. In fact, it is a plot of the Morse potential, which contains a weaker attractive and a very strong, repulsive constituent, localized at the core
52
Semiconductors for Micro and Nanosystem Technology
Elastic Properties: The Stressed Uniform Lattice
E ( r ) = D e ( 1 – exp [ – β ( r – r eq ) ] )
2
(2.10)
The potential energy for bond formation D e and the equilibrium bond length r eq depend on the constituent atoms, and may be obtained by experiment. The parameter β controls the width of the potential well, i.e., the range of the interparticle forces. For covalent crystals, such as silicon, this picture is too simplistic. The tetrahedral structure of the orbitals forms bonds that can also take up twisting moments, so that, in addition to atom pair interactions, also triplet and perhaps even larger sets of interacting atoms should be considered. A threeatom interaction model that accounts well for most thermodynamic quantities of Si appears to be the StillingerWeber potential [2.8], which, for atom i and the interaction with its nearest neighbors j , k , l and m is 1 E SiSi(r i, r j, r k, r l, r m) =  [ E 2(r ij) + E 2(r ik) + E 2(r il) + E 2(r im) ] 2 (2.11) + E 3(r ij, r ik, θ jik) + E 3(r im, r ik, θ mik) + E 3(r il, r im, θ lim) + E 3(r ij, r im, θ jim) + E 3(r ij, r il, θ jil) + E 3(r il, r ik, θ lik) In this model, the twoatom interaction is modelled as E 2(r ij) EG ( H e =
–p
– r ij ⁄ a
–q
–1
) exp ( ( r ij ⁄ a – c ) )
0
r ij ⁄ a < c
(2.12)
r ij ⁄ a > c
and the threeatom interaction by E 3(r ij, r ik, θ jik) –1 r ik r –1 Eλ exp γ ij – c +  – c a a = 1 2 × cos ( θ jik ) +  3 0
, r ij ⁄ a < c (2.13)
otherwise
Semiconductors for Micro and Nanosystem Technology
53
The Crystal Lattice System
For silicon, this model works well with the following parameters: G = 7.0495563 , H = 0.60222456 , p = 4 , q = 0 , λ = 21 , γ = 1.2 , the cutoff radius c = 1.8 , the “lattice” constant – 19 a = 0.20951nm and the bond energy E = 6.9447 ×10 J ⁄ ion . Note that in the above r ij = r i – r j . Linearization
We assume that the atoms of the crystal always remain in the vicinity of their lattice positions, and that the distance they displace from these positions is “small” when measured against the lattice constant a , see Figure 2.18. This is a reasonable assumption for a solid crystal at typical k uk rk = Rk + uk
i
Rk
Figure 2.18. Instantaneous snapshot of the atom positions of a regular square lattice with respect to their average lattice site positions. On the right is shown the relation between the lattice position vector R k , the atom position vector r k and the atom displacement vector u k for atom k. The shading around atom i indicates how the interatom interaction strength falls off as a function of distance.
operating temperatures; the covalent and ionic bonds are found to be strong enough to make it valid.
54
Semiconductors for Micro and Nanosystem Technology
Elastic Properties: The Stressed Uniform Lattice
Linearized Potential Energy
To illustrate the derivation of the elastic energy in terms of the strain and the elastic constants of the crystal, we will use an interatomic potential that only involves twoatom interactions. For a more general derivation, see e.g. [2.1]. Denote the relative vector position of atom i by u i , and its absolute position by r i = R i + u i , where R i localizes the regular lattice site. For a potential binding energy E between a pair of atoms as depicted in Figure 2.17 (II), we form the potential energy of the whole crystal with 1 U = 2
N
N
∑∑
1 E ( r i – r j ) = 2
N
N
∑ ∑ E(R – R i
j
+ ui – u j )
i=1j=1
i=1j=1
1 = 2
N
.
N
∑ ∑ E(R
ij
(2.14)
+ u ij )
i=1j=1
where R ij = R i – R j and u ij = u i – u j . The factor 1 ⁄ 2 arises because the double sum counts each atom pair twice. We expand the energy about the lattice site R ij using the Taylor expansion for vectors 1 2 E ( R ij + u ij ) = E ( R ij ) + ( u ij ⋅ ∇ )E ( R ij ) +  ( u ij ⋅ ∇ ) E ( R ij ) + … (2.15) 2 because of the assumption that the atom displacements u i and hence n their differences u ij are small. The terms ( u ij ⋅ ∇ ) E ( R ij ) must be read n as ( u ij ⋅ ∇ ) operating n times on the positiondependent energy E evaluated at the atom position R ij . Applying (2.15) to (2.14) we obtain 1 U = 2
N
N
∑∑
1 E ( R ij ) + 2
∑ ∑ (u
N
∑∑u
ij
• ∇E ( R ij )
i=1j=1
i=1j=1 N N
1 + 4
N
(2.16)
2
ij
• ∇ ) ( E ( R ij ) ) + …
i=1j=1
The ﬁrst term in (2.16) is a constant for the lattice, and is denoted by U o . The second term is identically zero, because the energy gradient is evaluated at the rest position of each atom where by deﬁnition is must be zero
Semiconductors for Micro and Nanosystem Technology
55
The Crystal Lattice System
1 2
N
N
∑∑u
ij
• ∇E ( R ij ) = 0
(2.17)
i=1j=1
This leaves us with the zeroth and second and higher order terms 1 U = U o + 4
N
N
∑ ∑ (u
2
ij
• ∇ ) E ( R ij ) + …
(2.18)
i=1j=1
The ﬁrst term in (2.18) is the energy associated with the atoms at the lattice positions, i.e., at rest, and represents the datum of energy for the crystal. The second term is the harmonic potential energy, or the smalldisplacement potential energy. When it is expanded, we obtain 1 h U = 4
N
N
∑∑u
ij
• ∇( ∇E ( R ij ) ) • u ij
(2.19)
i=1j=1
Elasticity Tensor
Equation (2.19) illustrates two terms, the deformation felt between two sites u ij , and the second derivative of the interatomic potential at zero deformation ∇( ∇E ( R ij ) ) . The second derivative is the “spring constant” of the lattice, and the deformation is related to the “spring extension”. We can now go a step further and write the harmonic potential energy in terms of the elastic constants and the strain. Moving towards a continuum view, we will write the quantities in (2.19) in terms of the position R i alone. Consider the term ∇[ ∇E ( R ij ) ] = ∇[ ∇E ( R i – R j ) ] . We expect E ( R ij ) to fall off rapidly away from R i when R j is far removed, so that for the site R i , most of the terms in (2.19) in the sum over j are effectively zero. To tidy up the notation, we denote D ( R i ) αβ as the components of the dynamical tensor D ( R i ) = ∇[ ∇E ( R ij ) ] . The remainder of the sites R j are close to R i , making R ij small, so that we are justiﬁed in making an expansion of the components of D ( R ij ) about R i D ( R ij ) αβ = D ( R i ) αβ + ∇ { D ( R i ) αβ } • R ij + …
56
Semiconductors for Micro and Nanosystem Technology
(2.20)
Elastic Properties: The Stressed Uniform Lattice
for which we only keep the leading term. We now apply a similar series expansion to the term u j , because we expect it to vary little in the vicinity of R i , and from now on we do not consider atom sites that are far away, to obtain u j = u i + R ij • ∇u i(R i) + …
(2.21)
Taking the ﬁrst righthandside term of (2.20) and the ﬁrst two terms of (2.21), and inserting these into (2.19), we obtain N
1 h U = – 4
N
∑ ∑ (R
T
ij
• ∇u i ) • D ( R i ) • ( R ij • ∇u i )
(2.22)
i=1j=1
The result of (2.22) can now be rewritten again in terms of the original quantities, to give N
1 h U = – 4
∑
N T
( ∇u i ) :
i=1
1 = – 2
∑ {R
ij D ( R i )R ij } : ∇u i
j=1
(2.23)
N
∑ ( ∇u ) :F(R ): ∇u T
i
i
i
i=1
The rank four elastic material property tensor F(R i) in the vicinity of the lattice site R i is deﬁned as 1 F(R i) = 2
N
∑ (R
ij D ( R i )R ij )
(2.24)
j=1
in terms of the crystal constituent positions and the resulting net interatom binding energy. We expect this tensor to be translationally invariant with respect to the lattice. Therefore, we can now move from a discrete crystal description to the continuum, by considering the crystal as a collection of primitive cells of volume V with an average “density” of elastic material property in any particular unit cell to be E = F ⁄ V , so that we can replace the sum in (2.23) by an integral to obtain
Semiconductors for Micro and Nanosystem Technology
57
The Crystal Lattice System
1 T h U = –  ( ∇u i ) • E • ∇u i dV 2
∫
(2.25)
Ω
Strain
We now wish to bring the gradient of deformation ∇u , a vectorvalued ﬁeld over the crystal, in relation to the strain, which is a rank two tensorvalued ﬁeld. We consider Figure 2.19, where we follow the behavior of x P′ dx′ Q′′ X
P
dx Q
Figure 2.19. An arbitrary body before and after deformation. The points P and Q are “close” to each other.
two points P and Q before and after deformation. The points are chosen to be close to each other, and we assume that the body has deformed elastically, i.e., without cracks forming, and without plastically yielding. To a very good approximation, the movement of each point in the body can then be written as a linear transformation P′ = α o + ( δ + α ) • P
58
Semiconductors for Micro and Nanosystem Technology
(2.26)
Elastic Properties: The Stressed Uniform Lattice
where α o represents a pure translation and α a rotation plus stretch. Next, we consider what happens to the line element d x under the deformation ﬁeld u T
T
d x′ = Q′ – P′ = α o + ( δ + α ) • Q – ( α o + ( δ + α ) • P ) T
(2.27)
= d x + α • d x = d x + du T
We can rewrite du via the chain rule as du = ( ∇u ) • d x , thereby making the association α = ∇u , to ﬁnd that we can now rewrite the expression for d x' only in terms of the original quantities that we measure T
d x' = d x + ( ∇u ) • d x
(2.28)
We are interested in how the line element deforms (stretches), and for this we form an expression for the square of its length 2
T
T
T
T
T
( d x' ) = ( d x ) • d x + [ ( ∇u ) • d x ] • d x + ( d x ) • [ ( ∇u ) • d x ] T
T
T
+ [ ( ∇u ) • d x ] • [ ( ∇u ) • d x ] T
T
(2.29)
T
= ( d x ) • [ δ + ∇u + ( ∇u ) + ( ∇u ) • ∇u ] • d x T
T
Consider the argument [ δ + ∇u + ( ∇u ) + ( ∇u ) • ∇u ] . If the stretch is small, which we have assumed, then we can use 1 + s ≅ 1 + s ⁄ 2 , which deﬁnes the strain ε by 1 1 T T T ε =  [ ∇u + ( ∇u ) + ( ∇u ) • ∇u ] ≈  [ ∇u + ( ∇u ) ] 2 2
(2.30)
The components of the small strain approximation may be written as 1 ∂u α ∂u β + ε αβ = 2 ∂ xβ ∂ xα
(2.31)
The small strain is therefore a symmetric rank two tensor.
Semiconductors for Micro and Nanosystem Technology
59
The Crystal Lattice System
Crystal Energy in Terms of Strain
We return our attention to equation (2.25), where our goal is to rewrite h the harmonic crystal energy U in terms of the crystal’s strain. Clearly, h U should not be dependent on our choice of coordinate axes, and is therefore invariant with respect to rigidbody rotations. We now choose a deformation ﬁeld u = θ × R which simply rotates the crystal atoms from their lattice positions by a constant deﬁned angle θ . The gradient of this ﬁeld is ∇u = ∇θ × R + θ × ∇R = 0 , so that the energy associated with pure rotations is clearly zero. The gradient of u can always be written as the sum of a symmetric and an antisymmetric part T
T
∇u = ∇u s + ∇u a = [ ∇u + ( ∇u ) ] ⁄ 2 + [ ∇u – ( ∇u ) ] ⁄ 2
(2.32)
= (ε + κ) Note that ε = ε obtain
T
T
and κ = – κ . We substitute ε and κ into (2.25) to
1 T T T T h U = –  ( ε :E:ε + ε :E:κ + κ :E:ε + κ :E:κ ) dV 2
∫
(2.33)
Ω
for the harmonic energy of the crystal. Independent Elastic Constants
The elastic tensor E has inherent symmetries that can be exploited to simplify (2.33). We ﬁrst write an expression for the components of the tensor E, centered at site i, in cartesian coordinates
E(R i) αβγµ
1 = 2V
N
∑ ( R j=1
∂
ij ) α ∂x β
∂E ( R i )  ( R ij ) γ ∂x µ
(2.34)
Consider the argument of the sum. Clearly, E is symmetric with respect to the indices β and µ , since the order of differentiation of the energy with respect to a spatial coordinate is arbitrary. Furthermore, swapping T T α and γ also has no effect. Now look at the terms ε :E:κ and κ :E:ε in (2.33). They vanish because, due the above symmetries of E , T T ε :E:κ = – κ :E:ε . Finally, because the antisymmetric strain κ repreT sents a pure rotation, the last term κ :E:κ in (2.33) must also vanish. As
60
Semiconductors for Micro and Nanosystem Technology
Elastic Properties: The Stressed Uniform Lattice
a consequence, the tensor E must be symmetric with respect to its ﬁrst and second pairs of indices as well, because it now inherits the symmetry of the symmetric strain. Thus we obtain the familiar expression for the elastic energy as 1 T h U = –  [ ε :E(R):ε ] dV 2
∫ V
N
3 1 T 1 = –  ε : ( R – R j ) D ( R ) ( R – R j ) :ε dR 2V 2 V j=1
(2.35)
∑
∫
Of the possible 81 independent components for the fourth rank tensor E, only 21 remain. We can organize these into a 6 × 6 matrix C if the following six index pair associations are made: E ( ij ) ( kl ) ≡ C ( m ) ( n ) 11 → 1 23 → 4
ij → m 22 → 2 31 → 5
kl → n 33 → 3 12 → 6
(2.36)
In order to obtain analog relations using the reduced index formalism, we have to specify the transformation of the stress and strain as well. For the stress we can use the same index mapping as in (2.36) σ ij ≡ s m 11 → 1 23 → 4
ij → m
22 → 2 31 → 5
33 → 3 12 → 6
(2.37)
For the strain, however, we need to combine the index mapping with a scaling e 1 = ε 11
e 2 = ε 22
e 3 = ε 33
e 4 = 2ε 23
e 5 = 2ε 31
e 6 = 2ε 12
(2.38)
In this way, we retain the algebraic form for the energy terms
Semiconductors for Micro and Nanosystem Technology
61
The Crystal Lattice System
1 1 T 3 T 3 h U = –  [ e • C(R) • e ] dR = –  [ e • s ] dR 2 2
∫
∫
(2.39)
V
V
The further reduction of the number of independent elastic coefﬁcients now depends on the inherent symmetries of the underlying Bravais lattice. Silicon has a very high level of symmetry because of its cubic structure. The unit cell is invariant to rotations of 90° about any of its coordinate axes. Consider a rotation of the xaxis of 90° so that x → x , y → z and z → – y . Since the energy will remain the same, we must have that C 22 = C 33 , C 55 = C 66 and C 21 = C 31 . By a similar argument for rotations about the other two axes, we obtain that C 11 = C 22 = C 33 , C 21 = C 31 = C 23 and C 44 = C 55 = C 66 . Since the other matrix entries experience an odd sign change in the transformed coordinates, yet symmetry of C is required, they must all be equal to zero. To summarize, Si and other cubicsymmetry crystals have an elasticity matrix with the following structure (for coefﬁcient values, consult Table 2.1) but with only three independent values: C 11 C 12 C 12 C 12 C 11 C 12 C =
C 12 C 12 C 11
(2.40) C 44 C 44 C 44
C can be inverted to produce S with exactly the same structure and the following relation between the constants: –1
–1
( S 11 – S 12 ) = ( C 11 – C 12 ) –1 ( S 11 + 2S 12 ) = ( C 11 + 2C 12 )
S 44 = C 44
(2.41)
The bulk modulus B and compressibility K of the cubic material is given by
62
Semiconductors for Micro and Nanosystem Technology
Elastic Properties: The Stressed Uniform Lattice
1 1 B =  ( C 11 + 2C 12 ) = 3 K
(2.42)
Isotropic materials have the same structure as (2.40) but with only two independent constants. In the literature, however, no less that three notations are common. Often engineers use the Young modulus E and Poisson ratio ν , whereas we ﬁnd the Lamé constants λ and µ often used in the mechanics literature. The relations between the systems are summarized by: C 11 – C 12  = µ C 44 =  2 Eν C 11 = λ + 2µ C 12 =  ( 1 + ν ) ( 1 – 2ν ) E(1 – ν) E C 11 =  C 44 = ( 1 + ν ) ( 1 – 2ν ) 2(1 + ν) λ µ ( 3λ + 2µ ) ν = E =  2(λ + µ) λ+µ C 11 – 2C 44 C 44 ( 3C 11 – 4C 44 ) ν =  E = 2 ( C 11 – C 44 ) C 11 – C 44 C 12 = λ
(2.43)
The α Quartz crystal has the following elastic coefﬁcient matrix structure (for coefﬁcient values, consult Table 2.1): C 11 C 12 C 12 C 14 C 12 C 11 C 12 – C 14 C Quartz =
C 12 C 12 C 11 C 14 – C 14
(2.44) C 44 C 44 C 44
Semiconductors for Micro and Nanosystem Technology
63
The Crystal Lattice System
2.4 The Vibrating Uniform Lattice The elastic, springlike nature of the interatomic bonds, together with the massive atoms placed at regular intervals; these are the items we isolate for a model of the classical mechanical dynamics of the crystal lattice (see Box 2.3 for brief details on Lagrangian and Hamiltonian mechanics). Here we see that the regular lattice displays unique new features unseen elsewhere: acoustic dispersion is complex and anisotropic, acoustic energy is quantized, and the quanta, called phonons, act like particles carrying information and energy about the lattice.
2.4.1 Normal Modes As we saw in Section 2.3, an exact description of the forces between the atoms that make up a crystal are, in general, geometrically and mathematically very complex. Nevertheless, certain simpliﬁcations are possible here and lead both to an understanding of what we otherwise observe in experiments, and often to a fairly close approximation of reality. We assume that:
• The atoms that make up the lattice are close to their equilibrium positions, so that we may use a harmonic representation of the potential binding energy about the equilibrium atom positions. The spatial gradient of this energy is then the positiondependent force acting on the atom, which is zero when each atom resides at its equilibrium position.
• The lattice atoms interact with their nearest neighbors only. • The lattice is inﬁnite and perfect. This assumption allows us to limit our attention to a single WignerSeitz cell by assuming translational symmetry.
• The bound inner shell electrons move so much faster than the crystal waves that they follow the movement of the more massive nucleus that they are bound to adiabatically.
64
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
Box 2.3. A Brief Note on Hamiltonian and Lagrangian Mechanics. Hamilton’s Principle. Hamilton’s principle states that the variation of the action A, also called the variational indicator, is a minimum over the path chosen by a mechanical system when proceeding from one known conﬁguration to another δA
t2 t1
= 0
(B 2.3.1)
The Action. The action is deﬁned in terms of the lagrangian L and the generalized energy sources Ξ j ξ j of the system A =
t2
∫t
1
n
L+
∑ Ξ jξ j
dt
(B 2.3.2)
j=1
where Ξ j is the generalized force and ξ j the generalized displacement The Lagrangian. The mechanical Lagrangian of a system is the difference between its kinetic coenergy T ∗ ( ξ˙ j, ξ j, t ) (the kinetic energy expressed in terms of the system’s velocities) and its potential energy U ( ξ j, t ) L M ( ξ˙ j, ξ j, t ) = T ∗ ( ξ˙ j, ξ j, t ) – U ( ξ j, t ) (B 2.3.3) In general, the lagrangian for a crystal is written in terms of three contributions: the mechanical (or matter), the electromagnetic ﬁeld and the ﬁeldmatter interaction L =
∫ ( L M + LF + LI ) dV
(B 2.3.4)
V
1 L M =  ( ρu˙ + ε • C • ε ) 2
(B 2.3.5) 1 A˙ ˙ L F =  ( E + B ) L I =  – qψ c 2 Generalized Energy Sources. This term groups all external or nonconservative internal sources
(sinks) of energy in terms of generalized forces Ξ j and the generalized displacements ξ j . Generalized Displacements and Velocities. For a system, we establish the m independent scalar m degrees of freedom d ∈ ℜ required to describe its motion in general. Then we impose the p constraint equations B • d = 0 that specify the m required kinematics (the admissible path in ℜ ). This reduces the number of degrees of freedom by p, and we obtain the n = m – p generalized scan m lar displacements ξ ∈ ℜ ⊃ ℜ of the system. The generalized velocities are simply the time rate of change of the generalized displacements, ξ˙ = dξ ⁄ dt . Lagrange’s Equations. An immediate consequence of (B 2.3.2) is that the following equations hold for the motion d ∂L ∂L = Ξj – d t ∂ ξ˙ j ∂ ξ j
(B 2.3.6)
These are known as the Lagrange equations of motion. For a continuum, we can rewrite (B 2.3.6) for the Lagrange density as d ∂L d ∂L ∂L   =  –  dt ∂ x˙ j ∂ x j d Xk ∂(∂ x j ⁄ ∂ Xk)
(B 2.3.7)
In the continuum crystal lagrangian the variables X represent the material coordinates of the undeformed crystal; x the spatial coordinates of the deformed crystal. The Lagrange equations are most convenient, because they allow us to add detail to the energy expressions, so as to derive the equations of motion thereafter in a standard way.
• The valence electrons form a uniform cloud of negative space charge that interacts with the atoms.
Semiconductors for Micro and Nanosystem Technology
65
The Crystal Lattice System
Normal Modes
Normal modes are the natural eigenshapes of the mechanical system. We already know these from musical instruments: for example from the shapes of a vibrating string (onedimensional), the shapes seen on the stretched surface of a vibrating drum (twodimensional), or a vibrating bowl of jelly (threedimensional). Normal modes are important, because they are orthogonal and span the space of the atomic movements and thereby describe all possible motions of the crystal. To obtain the normal modes of the crystal, we will assume timedependent solutions that have the same geometric periodicity of the crystal. We will now derive an expression for the equations of motion of the crysh tal from the mechanical Lagrangian L M = T ∗ – U (see Box 2.3.) From h T the previous section we have that U = 1 ⁄ 2 ( ε :E:ε ) dV . The kinetic V coenergy is added up from the contributions of the individual atoms
∫
1 T ∗ = 2
n
∑ mr˙
2 i
(2.45)
i=1
As for the potential energy, this sum can also be turned into a volume integral, thereby making the transition to a continuum theory. We consider a primitive cell of volume V 1 T ∗ = 2
n
1 2 m  r˙ V = V i 2
∑
n 2 i
i=1
i=1
1
∑ ρr˙ V ≅ 2 ∫ ρr˙ dV 2 i
(2.46)
V
Thus we have for the mechanical Lagrangian that LM =
∫L
M dV
V
LM
1 2 T =  ( ρr˙i – ε :E:ε ) dV , with 2
∫ V
1 2 T =  ( ρr˙i – ε :E:ε ) 2
(2.47)
The continuum Lagrange equations read [2.7] ∂L d d ∂L ∂L   =  –  dt ∂x˙ j ∂x j d X k ∂ ( ∂x j ⁄ ∂X k )
66
Semiconductors for Micro and Nanosystem Technology
(2.48)
The Vibrating Uniform Lattice
where we have chosen the coordinates X to describe the undeformed conﬁguration of the crystal, and x the coordinates in the deformed crystal, see Figure 2.19. 1D Monatomic Dispersion Relation
The complexity in applying the lagrangian formulation to a general 3D crystal can be avoided by considering a 1D model system that demonstrates the salient features of the more involved 3D system. A large 1D lattice of N identical bound atoms are arranged in the form of a ring by employing the Bornvon Karmann boundary condition, i.e., u ( N + 1 ) = u ( N ) . From equation (2.31), the strain in the 1D lattice is simply 1 du T ε 11 =  ( ∇u + ∇u ) = 2 dX
(2.49)
which gives a potential energy density of 1 du 2 U =  E  2 dX
(2.50)
where u is the displacement of the atom from its lattice equilibrium site and E is the linear Young modulus of the interatomic bond. Note that we only consider nearestneighbour interactions. The kinetic coenergy density is 1 2 * T =  ρu˙ 2
(2.51)
where the mass density is ρ = m ⁄ a for an atomic mass m and interatomic spacing a . The lagrangian density for the chain is the difference between the kinetic coenergy density and the potential energy density, * L = T – U . Note that u = X – x and hence that ∇u = Id – ∇x and u˙ = – x˙ . We insert the lagrangian density in equation (2.48) to obtain d du ρu˙˙ = – E   dX dX
Semiconductors for Micro and Nanosystem Technology
(2.52)
67
The Crystal Lattice System
Since the potential energy is located in the bonds and not the lattice site, and therefore depends on the positions of the neighboring lattice sites, 2 2 the term d u ⁄ d X is replaced by its lattice equivalent for the lattice site 2 i ( 2u i – u i – 1 – u i + 1 ) ⁄ a . This ﬁnite difference formula expresses the fact that the curvature of u at the lattice site i depends on the nextneighbor lattice positions. This step is necessary for a treatment of waves with a wavelength of the order of the interatomic spacing. If we use the simpler site relation, we only obtain the long wavelength limit of the dispersion relation, indicated by the slope lines in Figure 2.20. We now look for solutions, periodic in space and time, of the form u ( X, t )
X = ia
= exp [ j ( kX – ωt ) ]
X = ia
(2.53)
which we insert into equation (2.52) and cancel the common exponential E 2 – ρω = – 2 ( 2 – exp [ kia ] – exp [ – kia ] ) a
(2.54)
Reorganizing equation (2.54), we obtain ω =
ka E 2E ( 1 – cos [ ka ] )  = 2 2 sin 2 2 ρa ρa
(2.55)
Equation (2.55) is plotted in Figure 2.20 on the left, and is the dispersion relation for a monatomic chain. The curve is typical for an acoustic wave in a crystalline solid, and is interpreted as follows. In the vicinity where ω is small, the dispersion relation is linear (since sin [ ka ⁄ 2 ] ≈ ka ⁄ 2 ) and the wave propagates with a speed of E ⁄ ρ as a linear acoustic wave. As the frequency increases, the dispersion relation ﬂattens off, causing the speed of the wave ∂ω ⁄ ∂k to approach zero (a standing wave resonance). 1D Diatomic Dispersion Relation
Crystals with a basis, i.e., crystals with a unit cell that contains different atoms, introduce an important additional feature in the dispersion curve. We again consider a 1D chain of atoms, but now consider a unit cell containing two different atoms of masses m and M .
68
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
unit cell = a
unit cell = a
slope = 0 ω(k)
v
ω(k)
e=
v
slope =
Optical branch
slop
Acoustic branch Acoustic branch π a
π – a
X
∆
Γ
∆
π a
π – a
k
X
∆
X
Γ
∆
k
X
Figure 2.20. The monatomic and diatomic onedimensional chain lattices lend themselves to analytical treatment. Depicted are the two computed dispersion curves with schematic chains and reciprocal unit cell indicated as a gray background box. Γ is the symmetry point at the origin, ∆ the symmetry point at the reciprocal cell boundary. Only nearestneighbor interactions are accounted for.
The kinetic coenergy is added up from the contributions of the individual atoms 1 T ∗ = 2
n, 2
∑ m u˙
2 α iα
(2.56)
iα
The index α counts over the atoms in an elementary basis cell, and the index i counts over the lattice cells. Similarly, the bond potential energy is dependent on the stretching of the interatom bonds 1 U = 4
n, 2 , n , 2
∑
iα, βj
E αiβj 2  ( u iα – u jβ ) a
Semiconductors for Micro and Nanosystem Technology
(2.57)
69
The Crystal Lattice System
The restriction to nextneighbor interactions and identical interatomic force constants yields the following equations of motion when the expressions (2.56) and (2.57) are inserted into the Lagrange equations E mu˙˙im = –  ( 2u im – u iM – u ( i – 1 )M ) a
(2.58a)
E Mu˙˙iM = –  ( 2u iM – u ( i + 1 )m – u im ) a
(2.58b)
At rest the atoms occupy the cell positions (due to identical static forces) ( i – 1 ⁄ 4 )a and ( i + 1 ⁄ 4 )a . Hence we choose an harmonic atom displacement ansatz for each atom of the form 1 1 u im =  c m exp j ka i –  – ωt 4 m
(2.59a)
1 1 u iM =  c M exp j ka i +  – ωt 4 M
(2.59b)
The second ansatz can be written in terms of u im u iM =
ka m cM   exp j  u im 2 M cm
(2.60)
Equations (2.59b) and (2.60) are now inserted into (2.58a). Eliminating common factors and simplifying, we obtain an equation for the amplitudes c m and c M ka 2E 2E 2 – ω m –  cos  2 a m a M
cm
= 0
(2.61)
c ka 2E 2E 2 –  cos   – ω M M 2 a m a M This is an eigensystem equation for ω , and its nontrivial solutions are obtained by requiring the determinant of the matrix to be zero. Performing this, we obtain
70
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
ka 2 4 E 1 1 1 1 2 2 ω =   +  − +  +  –  sin  2 mM a m M m M
(2.62)
The two solutions are plotted in Figure 2.20 on the right. Discussion
The case when the two masses of the unitcell atoms differ only by a small amount, i.e., M = m + µ with µ small, is instructive. The optical and acoustic branches approach then each other at the edge of the reciprocal cell, i.e., at k = − + π ⁄ a . As the mass difference µ goes to zero, the lattice becomes a monatomic lattice with lattice constant a ⁄ 2 , so that the branches touch each other at the reciprocal cell edge. The interpretation of the two branches is as follows. For the lower branch, all the atoms move in unison just as for an acoustic wave, hence the name acoustic branch. In fact, it appears as a centerofmass oscillation. For the upper or optical branch, the center of mass is stationary, and the atoms of a cell only move relative to each other. Its name refers to the fact that for ionic crystals, this mode is often excited by optical interactions.
2D Square Lattice Dispersion Relation
The next construction shows the richness in structure that appears in the dispersion relation when an additional spatial dimension and one level of interaction is added to the 1D monatomic lattice. It serves as an illustration that the anisotropy of the interatomic binding energy enables more involved crystal vibrational modes and hence additional branches in the dispersion curves. At the same time it shows that most of the essential features of the expected structure is already clear from the simple 1D models. The model considers a 2D monatomic square lattice, and includes the interaction of the four nearest and four nextnearest neighboring lattice atoms, i.e., 8 interactions in all. Furthermore, the forces are assumed to be linear (the harmonic assumption) and the nextnearest neighbor spring
Semiconductors for Micro and Nanosystem Technology
71
The Crystal Lattice System
stiffnesses are taken to be f = 0.6 times the stiffnesses of the nearest neighbor bonds.
a
8
4
7
a
Figure 2.21. Model for a 2D monatomic square lattice. The atom numbers are markers for the derivation of the equations of motion.
5
1
3
9
2
6
Following the discussion for the linear lattices, we formulate the equations of motion as 2
mu˙˙αi = –
∑
β=1
∂U  = – ∂u βi
n
2
∑ ∑D
αβij
u βj , α = 1, 2 ,
j = 1β = 1
i = 1, 2, …, n
(2.63)
where the dynamical matrix D αβij represents the stiffness of the bond between atom sites i and j and between the directions α and β . The current model has a nineatom 2D interaction, for which we can use an 18 × 18 stiffness matrix. The nonzero unique elements of the matrix are E d 1 = D 1115 = D 2214 = D 1113 = D 2212 = – a
(2.64a)
fE d 2 = D 1119 = D 2218 = D 1117 = D 2216 = – a
(2.64b)
Equation (2.63) thus becomes fE E mu˙˙1 =  ( 4u 1 – u 5 – u 3 – u 2 – u 4 ) +  ( 4u 1 – u 9 – u 6 – u 7 – u 8 ) (2.65) a a We make an harmonic ansatz for the atom displacement of the form
72
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
u p = c exp { j [ ( pk x a + qk y a ) – ωt ] }
(2.66)
We can write the ansatz for any neighboring atom in terms of the central atom. For a parallel and diagonal atom we obtain u i, j = c exp { j { [ ( i – 1 )k x a + jk y a ] – ωt } } = u i, j e
– jk x a
u i – 1, j – 1 = c exp { j { [ ( i – 1 )k x a + ( j – 1 )k y a ] – ωt } } = u i, j e
(2.67)
– j(kxa + kya)
which, when inserted into (2.65) becomes – jk a jk a – jk a jk a E 2 – ω mc = c  [ ( 4 – e x – e x – e y – e y ) a
+ f (4 – e
– j(kxa + kya)
–e
– j(– kxa + kya)
–e
j(kxa + kya)
–e
– j(kxa – kya)
(2.68) )]
This single parameter eigenvalue equation has two solutions – jk a jk a – jk a jk a E 2 ω =  [ 4 – e x – e x – e y – e y am
+ f (4 – e
– j(kxa + kya)
–e
– j(– kxa + kya) jφ
Using the identity cos φ = ( e + e above to
–e – jφ
j(kxa + kya)
–e
– j(kxa – kya)
(2.69) )]
) ⁄ 2 we transform the equation
E −  { [ 4 – cos ( 2k x a ) – cos ( 2k y a ) ] ω = + am f [ 4 – cos ( 2k x a ) cos ( 2k y a ) ] } ]
1 2
(2.70)
The dispersion relation, equation (2.70), represents two ω surfaces in ( k x, k y ) space, and are plotted in Figure 2.22. Because not only nearest, but also next nearest neighbor interactions are included, the upper dispersion surface shows a new feature, in that the maximum is not at the boundary of the primitive cell, i.e., its gradient is zero in the interior of the cell.
Semiconductors for Micro and Nanosystem Technology
73
The Crystal Lattice System
ω ( k x, k y )
ky
π π ,  a a M
Σ Γ
π –π , –  a a
Z
∆
X kx
ky (a)
ky
π π , –  a a
(b)
kx
Figure 2.22. Acoustic dispersion branch surfaces ω ( k x, k y ) for a monatomic lattice with nearest and nextnearestatom linear elastic interaction. (a) One quarter of the surfaces are omitted to illustrate the inner structure. (b) The contours of the upper and lower surfaces. The interatom forces have a ratio of β = 0.6 .
By now the general method should become clear: the equations of motion, (2.63), written in terms of the discrete interatomic forces ∞ F 0 = ∑–∞ Γ p ⋅ u p acting on a typical lattice atom 0 , with a harmonic ansatz for the motion u p ( k ) = A exp { j [ k ⋅ r p – ωt ] } , leads to an eigenvalue equation. For a manyatom unit cell we obtain 2
ω B = D⋅B
(2.71) 1⁄2
for the amplitude eigenvectors B ( j ) = m j A ( j ) and eigenfrequencies ω . How to compute the dynamical matrix D is described, for the carbon lattice, in Box 2.4. Solving (2.71) for different values of k enables us to compute the phonon dispersion diagram shown in Figure 2.26 (but also see Figure 2.4). For Figure 2.4, a 6 × 6 low order approximation of the dynamical matrix was used that could easily be ﬁtted with the elastic
74
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
Box 2.4. Computing the carbon structure’s dynamical matrix. Atom Contributions. The dynamical matrix D describes the effect that perturbing the position of atom i has on the force acting on atom 0 , for all the interacting neighbors of atom 0 . Clearly this is a direct function of the crystal structure, so that we can write the dynamical matrix in terms of the bonding strengths between the adjacent sites. We now do this for the diamond lattice, depicted in Figure B2.4.1. From the viewpoint of atom 0 , we
{ 1 ⁄ 4, 1 ⁄ 4, – 1 ⁄ 4 } and { – 1 ⁄ 4, – 1 ⁄ 4, 1 ⁄ 4 } , at, r = 3 ⁄ 4 , and so on. The sets of equally distant neighbors are positioned in “onion shells” about atom 0 . For each of these sets we can write down a forceconstant tensor that is equal to the tensor product of its normalized position vector w.r.t. atom 0 . For example for the ﬁrst atom, the tensor equals 1 ⁄ 3 1 ⁄ 3 –1 ⁄ 3 Γ1 = γ 1 1 ⁄ 3 1 ⁄ 3 –1 ⁄ 3 –1 ⁄ 3 –1 ⁄ 3 1 ⁄ 3
(B 2.4.1)
and can be interpreted as follows: If atom i experiences a unit displacement in direction j , then atom 0 experiences a force in direction k of size ( i0 ) Γ jk . Each unique separation r l is associated with a force constant γ l . A complete formulation includes all force constant tensors and hence all neighboring atoms involved in an interaction with atom 0 .
Atom 0
The Dynamical Matrix. The net result of all atom interactions is computed from Figure B2.4.1: The structure of the diamond lattice w.r.t. the centered atom 0, marked by an arrow. Bookkeeping becomes critical. have 4 equally distant neighbors at the positions { 1 ⁄ 4, 1 ⁄ 4, – 1 ⁄ 4 } , { 1 ⁄ 4, – 1 ⁄ 4, 1 ⁄ 4 } ,
( i0 ) i ( k ⋅ r i ) 1 D jk = –  ∑ Γ jk e m i
(B 2.4.2)
The force constants are evaluated by comparing the longwavelength dynamical matrix with the values obtained from elasticity theory, (2.80).
constants of silicon. The qualitative agreement with the measured curve is fairly good, as all major features are represented. Phonon Density of States
A more useful form of the phonon density of states as a function of the phonon frequency D ( ω ) and not as a function of the wave vector coordinates. The density of states in k space is reasonably straightforward to formulate. For the case of a 1D monatomic lattice of length L with lattice constant a , it is the constant value w ( k ) = L ⁄ π for k ≤ π ⁄ a and zero otherwise. This amounts to saying that for each of the N atoms in
Semiconductors for Micro and Nanosystem Technology
75
The Crystal Lattice System
ω(k )
k Γ
∆
X
U, K
Σ
Γ
Λ
k L L
K
W
X
Figure 2.23. A computed phonon dispersion diagram for Silicon by the method described in the text. In this model, a dynamical matrix was used that only incorporates the nearest and next nearest neighbor atoms. In addition, a central force component was included so as to gain more realism. Qualitatively the shape closely resembles the diagram shown in Figure 2.4, which is based on measured values as well as a more realistic computation.
the chain there is one state, and in k space the density is N states per Brillouin zone volume. We expect the same result for 3D. The number of states D ( ω ) ω dω per frequency interval dω and at the frequency ω can be computed using w(k ) ∂k D ( ω ) ω dω = w ( k )  dω =  dω ∂ω ⁄ ∂k ω ∂ω ω
(2.72)
and so we see that the dispersion relation ω ( k ) is a prerequisite to compute the required density of states D ( ω ) = w ( k ) ⁄ ( ∂ω ⁄ ∂k ) . Before we look at a practical method with which to compute D ( ω ) for real crystals, we ﬁrst discuss an important structural feature, namely the singularities that occur when ∂ω ⁄ ∂k is zero. If we take a look at Figure 2.4, or simpler still, Figure 2.20, we see that at the symmetry points ∂ω ⁄ ∂k is either undeﬁned or zero. Thus we have that D ( ω ) either tends to inﬁnity
76
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
or shows a discontinuity. These are known as Van Hove singularities after their discoverer [2.14]. Phonon Density of States Computation Method
Since the density of states is constant in k space, the Walker calculation method [2.15] (also called the root sampling method) requires performing the following steps:
• Form a uniform grid in k space. Only consider a volume that is nonredundant, i.e., exploit all symmetries in the Brillouin zone of the crystal to reduce the size of the problem. Ensure that no grid points lie directly on a symmetry plane or on a symmetry line, as this would complicate the counting.
• For each point on the grid, solve (2.71) for the eigenfrequencies ω . • Compute ω max , the highest frequency anywhere on the grid. • Form a set of histogram bins from 0 to ω max for each separate branch of the computed dispersion curve, and calculate the histograms of branch frequencies found on the grid. That is, each histogram bin counts how many branch states occurred for a frequency lying within the bin’s interval.
• Identify the singular points on the histograms. Smoothen the histograms between the singular points and plot the resultant phonon density of states. The method requires enough k space points spread evenly over the Brillouin zone and histograms with smallenough bin widths for a realistic result. (The method can also be used to compute the density of electronic states E ( ω ) , from the electronic band structure E ( k ) , as discussed in Section 3.3). Applying the above algorithm to the linear chain of Section 2.4.1, we obtain the curves of Figure 2.24. Doing the same for the 2d lattice results in the densityofstates diagram of Figure 2.25. For the silicon dispersion diagram of Figure 2.23 we have numerically computed the density of states by the root sampling method presented in Figure 2.26.
Semiconductors for Micro and Nanosystem Technology
77
The Crystal Lattice System
ω
ω m = 0.1M
ω
M>m m = 0.1M
k ω
m = 0.1M k
ω
k ω
Dos
Dos
Dos
Figure 2.24. The computed phonon dispersion curves and densityofstates for the linear diatomic chain, for three mass ratios. The arrows show the positions of the Van Hove singularities. Also see Figure 2.20. For these plots ω was divided into 1000 bins, and 100000 evenlyspaced points in k space were used.
ω Figure 2.25. The computed phonon densityofstates for the 2D lattice. The arrows show the positions of the Van Hove singularities. Also see Figure 2.22. For this plot ω was divided into 1000 bins, and 360000 evenlyspaced points in k space were used.
Dos
As for the dispersion diagram, it shows the correct features of the density of states, but lacks realism due to the inadequacy of the dynamical matrix. Elastic Waves in Silicon
We now turn our attention to the classical mechanical equation of motion in a solid (2.52) and (2.63) in the long wavelength limit, but ignoring body forces
78
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
ω(k)
ω(k)
ω(k)
k
k
DOS
Figure 2.26. The computed phonon density of state diagram for a simplistic silicon model, shown together with the computed phonon dispersion diagram. Notice that peaks in the density of states diagram occur at positions where ∂ω ⁄ ∂k = 0 [2.13].
2
∂ u ρ 2 = ∇•σ = ∇•( C:ε ) ∂t
(2.73)
T
Remember that u = u 1 u 2 u 3 . It is simplest to ﬁrst evaluate σ = C:ε (here for a cubicsymmetry crystal) in the engineering notation of (2.38) and (2.40) C:ε
=
C 11 C 12 C 12
ε 11
C 11 ε 11 + C 12 ε 22 + C 12 ε 33
C 12 C 11 C 12
ε 22
C 12 ε 11 + C 11 ε 22 + C 12 ε 33
C 12 C 12 C 11
⋅
C 44 C 44 C 44
ε 33
=
C 12 ε 11 + C 12 ε 22 + C 11 ε 33
2ε 23
2C 44 ε 23
2ε 31
2C 44 ε 31
2ε 12
2C 44 ε 12 (2.74)
ant then to transform the result back to the usual tensor notation
Semiconductors for Micro and Nanosystem Technology
79
The Crystal Lattice System
C:ε C 11 ε 11 + C 12 ( ε 22 + ε 33 )
2C 44 ε 12
2C 44 ε 31
2C 44 ε 12
C 11 ε 22 + C 12 ( ε 11 + ε 33 )
2C 44 ε 23
2C 44 ε 31
2C 44 ε 23
C 11 ε 33 + C 12 ( ε 11 + ε 22 )
=
(2.75) We take the divergence of ∇•( C:ε ) , to obtain a ﬁrst version of the wave equation 2
∂ ( ε 22 + ε 33 ) ∂ε 11 ∂ u1 ∂ε 12 ∂ε 31 = C 11  + C 12  + 2C 44  + ρ 2 ∂x 1 ∂x 1 ∂x 2 ∂x 3 ∂t
(2.76a)
2
∂ ( ε 11 + ε 33 ) ∂ε 22 ∂ u2 ∂ε 12 ∂ε 23  + = C 11  + C 12  + 2C 44 ρ 2 ∂x ∂x ∂x 1 ∂x 3 2 2 ∂t
(2.76b)
2
∂ ( ε 11 + ε 22 ) ∂ε 33 ∂ u3 ∂ε 31 ∂ε 23 = C 11  + C 12  + 2C 44  + ρ 2 ∂x ∂x ∂x 1 ∂x 2 3 3 ∂t
(2.76c)
With the deﬁnition of strain (2.31) we obtain the ﬁnal form of the bulk lattice wave equation system for a cubicsymmetry crystal 2
2
2
2
2
2
2
2
2
2
2
2
2
2
2
2
2
2
∂ u 1 ∂ u 1 ∂ u2 ∂ u1 ∂ u1 ∂ u3 = C 11 + ( C 12 + C 44 ) +  + C 44  + ρ  2 2 2 ∂x ∂x ∂x ∂x 1 3 ∂x 22 1 2 ∂x 1 ∂t ∂x 3 (2.77a) ∂ u 2 ∂ u 2 ∂ u1 ∂ u2 ∂ u2 ∂ u3 = C 11 + ( C 12 + C 44 ) +  + C 44  + ρ  2 2 2 ∂x 2 ∂x 1 ∂x 2 ∂x 3 ∂x 21 ∂x 2 ∂t ∂x 3 (2.77b) ∂ u 3 ∂ u 3 ∂ u1 ∂ u3 ∂ u3 ∂ u2 +  + C 44  + ρ = C 11 + ( C 12 + C 44 )  2 2 2 ∂x 21 ∂x 3 ∂x 1 ∂x 3 ∂x 2 ∂t ∂x 3 ∂x 2 (2.77c) To ﬁnd the principal bulk modes, we assume a harmonic plane wave solution of the form
80
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
k⋅x u = Af ( τ ) , with τ = t – c
(2.78)
and unit vector k pointing in the direction of wave propagation, so that (2.77a) becomes an eigensystem 2
( Γ – ρc ) ⋅ A = 0
(2.79)
with the tensor Γ deﬁned for cubic materials such as silicon as 2
2
2
C 11 k 1 + C 44 ( k 2 + k 3 ) Γ =
( C 12 + C 44 )k 1 k 2 2 C 11 k 2
( C 12 + C 44 )k 1 k 2 ( C 12 + C 44 )k 1 k 3
+
2 C 44 ( k 1
+
( C 12 + C 44 )k 1 k 3
2 k3)
( C 12 + C 44 )k 2 k 3
( C 12 + C 44 )k 2 k 3 2
2
2
C 11 k 3 + C 44 ( k 1 + k 2 ) (2.80)
Equation (2.79) is also known as the Christoffel equation, and ﬁnding its eigenvalues using material parameters for silicon, over a range of angles, results in the slowness plots of Figure 2.27 [2.11]. Along the [ 100 ] family of silicon crystal axes, the principal wave velocities are c1 =
C 11 ⁄ ρ = 8433m ⁄ s ,
c2 = c3 =
C 44 ⁄ ρ = 5845m ⁄ s
(2.81a) (2.81b)
Along the [ 110 ] direction, we obtain the following results C 44 ⁄ ρ = 5845m ⁄ s
(2.82a)
( C 11 – C 12 ) ⁄ 2ρ = 4674m ⁄ s
(2.82b)
( C 11 + C 12 + 2C 44 ) ⁄ 2ρ = 9134m ⁄ s
(2.82c)
c1 = c2 = c3 =
2.4.2 Phonons, Speciﬁc Heat, Thermal Expansion The behavior of certain material properties, such as the lattice heat capacity at low and medium temperatures, can only be explained if we assume that the acoustic energy of lattice vibrations is quantized, a result indi
Semiconductors for Micro and Nanosystem Technology
81
The Crystal Lattice System
(a)
[ 001 ]
(b)
[ 001 ]
[ 111 ] Quasilongitudinal P wave
[ 010 ]
[ 010 ] [ 100 ] Shear polarization S wave
Quasishear S wave
Figure 2.27. The three computed slowness surfaces for silicon. These waves have differing velocities of propagation as shown in the ﬁgures. (a) The 3D plot of the quasi waves shows minima along the [ 111 ] axes. (b) Here we see that the shear polarization wave for silicon is isotropic, and hence a circle. The dotted line is a circle, provided for reference. –4 The inverse wave velocities at the crystal axes intersections are 1.119 ×10 s ⁄ m and –4 1.711 ×10 s ⁄ m . Also see Box 2.5.
cated in the previous section on the normal modes of the crystal. By performing a quantummechanical analysis of the lattice, essentially consisting of taking a Hamiltonian of the crystal and ﬁnding its stationary state (see 3.2.5), we ﬁnd that the vibrational energy is quantized for the various states as E j = —ω j .
(2.83)
The vibrational energy is also a travelling wave (see Box 2.1) which has a distinct momentum, so that p = —k .
82
Semiconductors for Micro and Nanosystem Technology
(2.84)
The Vibrating Uniform Lattice
Box 2.5. The characteristic surfaces of waves in anisotropic media [2.11]. For a general anisotropic medium we can write the orientationdependent strength of a plane wave as c(k) = c(k) k , k = 1
(B 2.5.1)
Thus c(k) ⋅ k = c(k) It is usual to set
(B 2.5.2)
k = ( sin θ cos φ, sin θ sin φ, cos θ ) (B 2.5.3) Equation (B 2.5.1) describes a closed surface called the velocity surface. We have seen that a general anisotropic medium supports three waves, two of which are quasishear transverse waves and one that is a quasiparallel normal wave. Thus we have a family of three wave surfaces. Inverting equation (B 2.5.1) we obtain L(k) = k ⁄ c(k) (B 2.5.4) so that c(k) ⋅ L(k) = 1 . Equation (B 2.5.4) describes a closed surface called the slowness surface. Again there are three surfaces corresponding to the different wave mode solutions. E
Normality. We now wish to form c (k) ⋅ d L(k) , for which we ﬁrst deﬁne the two arguments. The modal wave’s Poynting vector is
k ⋅ ∇ k c(k) δ k ∇ k L = ∇ k  =  – (B 2.5.8) 2 c(k) c(k) c(k) But ∇ k c(k) is nothing else than the group velocG ity of the wave c , which in turn equals to T 2 ( 2 ( A ⋅ C ): A ⋅ k ) ⁄ ( c(k)ρ A ) , so that we E deduce that c (k) ⋅ d L(k) = 0 . This means that the energy velocity is normal to the slowness surface. Complementarity. The scalar product of the energy velocity and the direction vector gives the magnitude of the wave velocity in that direction, E i.e., c (k) ⋅ k = c ( k ) . This follows from the Christoffel equation, (2.79). Hence we see that E c (k) ⋅ L(k) = 1 . Now consider the following construction E
E
d ( c (k) ⋅ L(k) ) = d c (k) ⋅ L(k) +
(B 2.5.9) c (k) ⋅ dL(k) = d c (k) ⋅ L(k) = 0 Inserting the deﬁnition for L(k) , we obtain that E
E
E
d c (k) ⋅ k = 0 , or, that the tangent of the velocity surface is normal to the propagation direction. The above ﬁndings are now summarized in.
C: ( A ⊗ A ) ⋅ k ∂f 2 P = – ( σ ⋅ u˙ ) =   (B 2.5.5) ∂τ c(k) dL
Together with the wave’s energy density 1 2 ∂f 2 E 0 =  ρ A  ∂τ 2 we form the energy velocity vector c E P 2C: ( A ⊗ A ) ⋅ k c (k) =  = 2 E0 c(k)ρ A Since dL = ∇ k L ⋅ dk , we obtain
dc
E
k
Slowness Surface
by (B 2.5.7)
E
L
(B 2.5.6) E
c
Wave Surface Figure B2.5.1: The basic geometric relations of the characteristic wave surfaces. Also refer to Figure 2.27 for the slowness surface of silicon.
Vibrational energy quanta follow the statistics of bosons, i.e., they are not subject to the Pauli exclusion principle that holds for fermions such as the electrons, so that Semiconductors for Micro and Nanosystem Technology
83
The Crystal Lattice System
1 1 〈 n j〉 =  =  , exp ( ( —ω j – µ ) ⁄ kT ) – 1 exp ( ( E j – µ ) ⁄ kT ) – 1
(2.85)
We will delay any further discussion of particle statistics to Chapter 5. Because of the similarity of this expression with the case of photons (quantized electromagnetic energy, see Section 5.2.4), the quantized crystal vibrations are called phonons. Phonons
The connection to the normal modes of the previous section is that the th excitation of the m mode (from branch s with wavevector k ) corresponds to saying that there exist m photons (from branch s with wavevector k ) in the crystal [2.1].
Heat Capacity
The vibrating crystal lattice is an internal energy store. A measure for this energy storage ability is the heat capacity at constant volume, deﬁned as ∂E ∂S C V = T  =  ∂T V ∂T V
(2.86)
in terms of the entropy S and the internal energy E . Classical statistical mechanics (SM), which treats the lattice as 3N classical linear harmonic oscillators, assigns an average of energy kT to each vibrational degreeoffreedom, from –E kBT
U
∂ ∫ e E dΓ = –  ln = 
∫
e
–E kBT
dΓ
1 ∂  kBT
∫e
–E kBT
dΓ
(2.87)
= 3N k B T = 〈 E〉 Classical and hence we obtain a simple expression for the heat capacity as ∂E –1 –1 C V =  = 3N k B ≈ 24 Jmol K ∂T V
84
Semiconductors for Micro and Nanosystem Technology
(2.88)
The Vibrating Uniform Lattice
The expression shows no temperature dependence, which turns out to be wrong for all but the very high temperatures. This classical result is due to Dulong and Petit. From classical mechanics (CM), we obtained the 3N normal modes of the crystal via a quadratic expression for the Hamiltonian (the harmonic approximation). In CM, any motion of the crystal is simply a linear combination of the normal modes, each with its characteristic frequency ω , without regard to the energy. A quantummechanical (QM) treatment of the linear harmonic oscillator, however, assigns each mode with allowed energy levels E = ( n + 1 ⁄ 2 )—ω , n = 1, 2, … . The internal energy must depend on how energy is absorbed into the quantized phonon levels. We calculate the energy of the ensemble of oscillators as a sum over the QM states Ei – kBT
∑
Ee i i  ≈ U equilibrium + U = E i
∑
Ei ⋅ e
– kBT
1
∑ 2 —ω ( k ) i
(2.89)
i
+
—ω ( k )
∑ E i
exp – i  – 1 kBT
from which we can evaluate the speciﬁc heat as CV =
∂
—ω ( k )
 ∑ E ∂T i
(2.90)
exp – i  – 1 kBT
This quantumcorrected model now depends on the temperature, as required. Since we know how to determine ω ( k ) , (2.90) can in principle be evaluated. A particularly simple QM model was worked out by Debye. It replaces the lattice’s dispersion relation with a simpliﬁed linear form, ω ( k ) = v s k , where v s is the scalar isotropic speed of sound in the crystal (the equation for the slope(s) in Figure 2.20). In addition, the Debye
Semiconductors for Micro and Nanosystem Technology
85
The Crystal Lattice System
temperature Θ D is introduced that characterizes the lowest temperature at which all modes of the crystal are being excited. After some algebraic manipulations (see e.g. [2.1], p. 458) we obtain the expression ΘD T
T 3 C v = 9N k B  Θ D
∫ 0
4 x
x e 2 dx x (e – 1)
(2.91)
Upon evaluation the Debye relation leads to the following rather awful but exact analytical expression (computed using Mathematica®) ΘD 4 T 1 C v = – 9N k B 4 15 exp  – 4 π  + T ΘD ΘD T 15 exp  – 1  T ΘD ΘD ΘD 4 T T 4 exp  π  + 60  ln 1 – exp  ΘD T T ΘD T T ΘD 60 exp   ln 1 – exp ΘD ΘD T
–
+
ΘD 2 T T ΘD 2 T 180  Li 2( exp  ) – 180 exp   Li 2( exp  ) – T ΘD ΘD T ΘD ΘD 3 T T ΘD 3 T 360  Li 3( exp  ) – 360 exp   Li 3( exp  ) + T ΘD ΘD T ΘD ΘD 4 T T ΘD 4 T 360  Li 4( exp  ) – 360 exp   Li 4( exp  ) T ΘD ΘD T ΘD (2.92) where Li m(z) is the polylogarithm function. It provides an excellent approximation of the speciﬁc heat over all temperature ranges, and is plotted in Figure 2.28. Anharmonicity
The harmonic potential is in fact a truncated series expansion model of the true crystal interatom potential, and as such is not capable of explaining all lattice phenomena satisfactorily. We brieﬂy discuss one important examples here: the expansion of the lattice with temperature.
86
Semiconductors for Micro and Nanosystem Technology
The Vibrating Uniform Lattice
C V J ⁄ moleK 20 Figure 2.28. The speciﬁc heat C V of a harmonic crystal versus T ⁄ Θ D computed using the Debye interpolation formula. The high temperature limit of DuLong and Petit is approximately 24 J ⁄ moleK .
10
0
T ΘD 0
1
2
3
The other important example, the lattice thermal conductivity, will be discussed in Section 7.1.2. Thermal Expansion
The thermal expansion coefﬁcient is deﬁned by 1 ∂P 1 ∂V =   α T =   3B ∂T ( V ) V ∂T ( P )
(2.93)
where B is the bulk modulus deﬁned as B = – V ( ∂P ⁄ ∂V ) ( T ) , and equal to the inverse of the compressibility, l is some length, T is the temperature, P is the pressure and V is the volume. From thermodynamics, we have that ∂F ∂U ∂S and F = U – TS =  , P = –  T  ∂V ( T ) ∂T ( V ) ∂T ( V )
(2.94)
for the entropy S , the internal energy U and the Helmholtz free energy F . Combining these, we can write the pressure only in terms of the internal energy, volume and temperature as ∂ P = –  U – T ∂V
T
∫
0
dT′ ∂  U ( T′, V )  T′ ∂T′
(2.95)
All that remains is to insert the expression (2.89) for the internal energy into (2.95), and then to insert this result into (2.93). Evaluating this Semiconductors for Micro and Nanosystem Technology
87
The Crystal Lattice System
expression is beyond our scope. It is important, however, to note that it we assume a harmonic crystal potential (and hence internal energy) then the thermal expansion coefﬁcient would vanish. If a fourthorder model is used (the third order expansion being unstable) we obtain
1 α = 3B
∑∑ k
i
1 ∂ ∂ –   —ω   ∂V k ∂T Ei  – 1 exp – k T
(2.96)
B
This expression is often simpliﬁed by the introduction of a Grüneisen parameter γ that absorbs the derivatives of the mode frequencies w.r.t the volume, and that exploits the similarities of (2.90) and (2.96), to yield α = γ c v ⁄ 3B .
2.5 Modiﬁcations to the Uniform Bulk Lattice Up to now we have considered the perfect crystal to be inﬁnitely extended in space, which enabled us to make a straightforward ansatz for the mechanical behavior of a crystal atom in the potential ﬁeld of the electrons. In reality semiconductor crystals are ﬁnite, subject to defects, and terminated by surfaces. Semiconductor manufacturing is performed for the most part by selectively growing and etching thin ﬁlm layers at the uppermost surface of a semiconductor wafer, and hence active devices include a variety of material interfaces. Since the real crystal has a modiﬁed structure, we will look at the implications for the phonons. Surface phonons are dealt with in Chapter 7. Point defects
When a single atom in the lattice is substituted by another atom type with different mass and/or a different binding force, the uniform lattice description is no longer valid. Qualitatively, new spatially localized phonon states become possible. These can be one of the following four cases:
88
Semiconductors for Micro and Nanosystem Technology
Modifications to the Uniform Bulk Lattice
• A: at a frequency higher than the optical branch, and, • B: close enough to the optical branch to cause a splitting of its levels; • C: between the optical an acoustic branch; • D: within the acoustic branch. The cases are illustrated in Figure 2.29. We now reconsider the diatomic A B
Figure 2.29. Positions of the four localized phonon states, due to point defects [2.12], on a 1D diatomic lattice densityofstates diagram.
Optical Branch
C D
Acoustic Branch
lattice, with masses M and m , of Section 2.4.1 but with the mass of one site slightly perturbed, i.e., replaced with a mass µ . The four cases are:
• µ < m < M , mass of type m is replaced; • m < µ < M , mass of type m is replaced, i.e., in the gap; • m < µ < M , mass of type M is replaced, i.e., in the gap; • m < M < µ , mass of type M is replaced. Introducing an Interface
The assumptions we have made about the bulk crystal lattice do not necessarily hold at the interface, and as a result we can expect certain modiﬁcations to the physical effects we have considered so far that should account for its presence. One reason why material surfaces and interfaces are important, is that we usually build devices on crystal surfaces; also, many effects that are useful take place at material interfaces. By an interface we denote that transition region between the bulk crystal and some other substance, whether it is a solid, liquid or gas. Usually the interface
Semiconductors for Micro and Nanosystem Technology
89
The Crystal Lattice System
is only a few atomic diameters thick, and if it separates the crystal from a liquid or gas, we usually denote it as the surface of the crystal. A new crystal surface can be formed by etching into an existing crystal, or by growing a crystal from a seed, or by cleaving an existing crystal along one of its planes. An interface can be created by depositing another material onto the crystal, or by performing a reaction on the crystal surface that results in another compound being formed (e.g., by oxidation). This section will only introduce a few important concepts. Surface physics is a large and active discipline and the interested reader is encouraged to refer to a specialized text such as [2.2]. Dangling Bond
Immediately after a crystal surface is formed in a vacuum by cleaving, the atoms at the surface have dangling bonds. In time, the atoms rearrange themselves to assume a more energetically favorable conﬁguration. For example, the atoms, still bound to the underlying bulk material, will relax to a lattice constant smaller (or larger) than the bulk value, to reﬂect the fact that the bonding forces are onesided in a direction normal to the surface. Furthermore, the surface could buckle in shape so as to enable the dangling bonds to create bonds with each other. In silicon, atoms on the surface can form a socalled 2 × 1 (or 7 × 7 ) reconstruction with π bonded chains [2.2], see Figure 2.30. In the atmosphere, we can expect various gas atoms and molecules to attach to the dangling bonds. For example, it appears that hydrogen preferentially bonds to silicon surfaces, a fact that inﬂuences for example the etch rate of silicon. We will consider a simple model of a crystal surface to describe the modiﬁcations to the bulk dispersion relation in Section 7.6.3.
Superlattices
A superlattice is a term used for any latticelike structure with a lattice constant larger than that of the underlying crystalline material. Thus, e.g., when a crystal surface forms atomic rearrangements due to relaxation effects, a superlattice is formed with a lattice constant that is often twice as large as before. Epitaxially formed heterostructures such as found in
90
Semiconductors for Micro and Nanosystem Technology
Summary for Chapter 2
1 Intermediate layer atom 2 Adatom
3 Dimer Atom 4 Rest Atom
1
3
2
4
(b) 1
3 4
2 (a)
(c)
Figure 2.30. (a) The Si 〈 111〉 7 × 7 reconstructed surface imaged with a scanning tunneling microscope. The overlay indicates the various atomic positions in the DAS layer. The pictures (b) and (c) to the right are for comparison purposes, and show the ﬁrst four silicon atom layers. (c) Shows a 3dimensional view of the ﬁrst four atom layers of the lattice.
quantumwell semiconductor lasers also represent superlattices. We expect the superlattice to have a local inﬂuence on the dispersion curve because additional waves are admitted with another wavelength [2.2], [2.16].
2.6 Summary for Chapter 2 The forces between the constituent atoms of a crystal lead to the pseudoparticle of lattice vibrational energy: the phonon. From this view, we obtain the dispersion curves for a solid with its different phonon branches. The acoustic phonons, in the long wavelength limit, are the elastic waves we know from a macroscopic viewpoint, and we completely recover the classical theory of elasticity. The high frequency opti
Semiconductors for Micro and Nanosystem Technology
91
The Crystal Lattice System
cal phonons explain why a solid lattice is able to interact with light. With the simpler harmonic model we already obtain useful expressions for the heat capacity and thermal expansion. In Chapter 7 we will see that for a realistic model of the heat conductivity, this model must be extended.
2.7 References for Chapter 2 2.1
Neil W. Ashcroft, N. David Mermin, Solid State Physics, Saunders College Publishing, Philadelphia (1988) 2.2 H. Lüth, Surfaces and Interfaces of Solid Materials, 3rd Ed., Springer Verlag, Berlin (1995) 2.3 MarieCatharin Desjonquères, D. Spanjaard, Concepts in Surface Physics, 2nd Ed., Springer Verlag, Berlin (1996) 2.4 Otfried Madelung, Introduction to SolidState Theory, SpringerVerlag, Heidelberg (1981) 2.5 Otfried Madelung, Semiconductors  Basic Data, SpringerVerlag, Heidelberg (1996) 2.6 Arokia Nathan, Henry Baltes, Microtransducer CAD, SpringerVerlag, Vienna (1999) 2.7 D. F. Nelson, Electric, Optic and Acoustic Interactions in Dielectrics, John Wiley and Sons, New York (1979) 2.8 Frank H. Stillinger, Thomas A. Weber, Computer Simulation of Local Order in Condensed Phases of Silicon, Phys. Rev. B, 31(8) (1985) pp. 5262–5271 2.9 Simon M. Sze, Physics of Semiconductor Devices, 2nd Ed., John Wiley and Sons, New York (1981) 2.10 Franklin F. Y. Wang, Introduction to Solid State Electronics, 2nd Ed., NorthHolland, Amsterdam (1989) 2.11 Abraham I. Beltzer, Acoustics of Solids, Springer Verlag, Berlin (1988) 2.12 R. W. H. Stevenson, ed., Phonons in Perfect Lattices and in Lattices with Point Defects, Scottish Universities Summer School 1965, Oliver & Boyd, Edinburgh (1966). Chapter 1, General Introduction, by C. Kittel, Chapter 2, Phonons in Perfect Lattices, by W. Cochran.
92
Semiconductors for Micro and Nanosystem Technology
References for Chapter 2
2.13 Ian Johnston, Graham Keeler, Roger Rollins and Steven Spicklemire, Solid State Physics Simulations, John Wiley & Sons, New York (1996) 2.14 Léon van Hove, The Occurrence of Singularities in the Elastic Frequency Distribution of a Crystal, Phys. Rev. 89(6) (1953) 11891193 2.15 C. B. Walker, XRay Study of Lattice Vibrations in Aluminium, Phys. Rev. 103(3) (1956) 547557 2.16 Peter Y. Yu, Manuel Cordona, Fundamentals of Semiconductors, Springer Verlag, Berlin (1996)
Semiconductors for Micro and Nanosystem Technology
93
Chapter 3 The Electronic System
Since the early days of discoveries on the nature of electrons, (we can note in hindsight), the world hasn’t looked back. One notable laboratory at Bell Laboratories, run by William Schockley, has brought us innumerable innovations to control and exploit the behavior of electrons in semiconductors, including the transistor, and establishing many of the key ideas used in semiconductor circuits today that, upon reading in one sitting, lets us amaze at how clear these pioneers already saw the end result. Subsequent industrial innovations have not let us down, engineering ever faster switching transistors and electronic circuits according to the famed “law” of Gordon Moore, whereby miniaturization and speedup doubles every one and a half years. The result: current laptop computers are as powerful as the supercomputer of the author’s student days (but much more reliable and comfortable to use!). Chapter Goal Electrons move through crystals in special ways, and the mechanism is dominated by quantum mechanics. The goal of this chapter is therefore to introduce two topics:
Semiconductors for Micro and Nanosystem Technology
95
The Electronic System
• Basic quantum mechanics; • The semiconductor electronic system, and the band structure of silicon. Chapter Roadmap
We start with the free electron, introducing the Schrödinger equation. Next, the electron is bound by a variety of potentials. The hydrogen atom represents the simplest quantummechanical model of an atom, with good predictive qualities. This leads up to the periodic potential, a model for the periodicallyplaced crystal atom potentials. This model naturally leads to the concepts of a forbidden band, and band splitting. The chapter wraps up with and expression for the effective mass of the bound electrons. In this chapter we take some space to explain the necessary mathematical instruments and physical concepts to understand the quantum nature of phenomena described in the book. You are strongly encouraged to carefully study the mathematical manipulations of wavefunctions, operators and all the objects described in this chapter. Moreover, you should freely work with all the objects and practise to manipulate them. Most of the time you will gain a deeper understanding, and of course there is no risk of doing any harm to them. The worst that can happen is that you might not ﬁnd any meaningful physical interpretation for what you did. For a detailed understanding of speciﬁc topics special literature is given in the references.
3.1 Quantum Mechanics of Single Electrons Quantum mechanics describes the fundamental properties of electrons [3.1], [3.2]. It tells us that both particlelike and wavelike behavior is possible. In a semiconductor both types of behavior are observable. The particle concept turns out to be an excellent description for a wide range of classical phenomena and the most common applications. Modern devices on the nanometer scale instead demonstrate the quantum nature
96
Semiconductors for Micro and Nanosystem Technology
The Electronic System
Interference Experiment
The interference pattern on the screen shows the dependence of the intensity on the acceleration bias for the electrons, which itself is a measure of the momentum of an electron. The fact that the electron waves follow the Bragg relation gives for the momentum and wavevector the relation p = —k , where — is the Planck constant. Thus we describe the electrons as a plane wave in the same way as we did for the lattice waves (Box 2.1). These waves have a frequency ω and a wavevector k and are characterized by the functions sin ( ωt – kx ) , cos ( ωt – kx ) , exp ( ωt – kx ) or linear combinations of them. An arbitrary linear combination Ψ ( x, t ) , in general, is a complex scalar ﬁeld. On the other hand, the particle’s position x, its momentum p, charge q and many other properties that may be determined by measurement are real quantities. Therefore, we need an interpretation of the wavefunction.
Probability Density
The square modulus of the wavefunction Ψ ( x, t ) 2 is interpreted as the probability density of ﬁnding an electron at time t at position x. Thus for a normalized wavefunction
∫ Ψ ( x, t )
Ω
2 dV
=
∫ Ψ∗ ( x, t )Ψ ( x, t ) dV
= 〈ΨΨ〉 = 1
(3.1)
Ω
holds, because the electron must be found with probability one somewhere in the physical domain Ω . We implicitly assumed that the wavefunction is squareintegrable, i.e., the integral over Ω exists. This is not necessarily the case, as we shall later when dealing with free electrons. 〈ΨΨ〉 = Ψ is called the norm of Ψ and (3.1) is the standard form for the numerical evaluation of the expectation values of operators. The shorthand notation given by the last term in angle brackets is known as the Dirac notation. Once we have deﬁned the probability density ρ ( x, x ) = Ψ∗ ( x, t )Ψ ( x, t )
(3.2)
we calculate its moments. Remember that for a real mass density the property corresponding to the ﬁrst moment with respect to the position
98
Semiconductors for Micro and Nanosystem Technology
Quantum Mechanics of Single Electrons
vector x is the center of mass. For the electron described in terms of a wavefunction it is the average value of its position 〈 xˆ 〉 =
∫ Ψ∗ ( x, t ) xˆ Ψ ( x, t ) = 〈Ψxˆ Ψ〉
(3.3)
Ω
In this case xˆ is called the position operator. We shall use ˆ to identify operators whenever we are not dealing with a special representation. In the position representation xˆ is a vector with cartesian components x, y and z. Expectation Values
The result of (3.3) gives the most probable position where to ﬁnd a particle. It is called the expectation value of the position operator. It is possible to calculate the expectation values of arbitrary functions of xˆ , such as the variance of the position, which gives us important information about the spreading of the wavefunction Var ( x ) = 〈 ( ∆ xˆ ) 2〉 = 〈Ψ( xˆ – 〈 xˆ 〉 ) 2 Ψ〉 = 〈Ψ( xˆ 2 – 〈 xˆ 〉 2 )Ψ〉
(3.4)
An illustrative example is shown in Figure 3.2, representing a oneψ( x)
σ
Figure 3.2. A Gaussianshaped wavefunction with its average value 〈 ψ ( x )〉 and variance σ .
〈 ψ ( x )〉 x
dimensional wavefunction at t = t 0 given by
Semiconductors for Micro and Nanosystem Technology
99
The Electronic System
( x – x 0 ) 2 1 1 / 2 exp – σ Ψ ( x, t 0 ) = ψ ( x ) =  ( 2π ) 1 / 4 4σ 2
(3.5)
For the wavefunction of type (3.5) σ 2 = 〈 ( ∆ xˆ ) 2〉 holds.The spatial wavefunction may be represented as a superposition of plane waves, i.e., as an inverse Fourier transform ∞
1 ψ ( x ) = 2π
∫ φ ( k ) exp ( ikx ) dk
(3.6)
–∞
The wavevector in (3.6) is the same as found in the momentum relation above. Position and Momentum Representations
ψ ( x ) we call the wavefunction in position representation, more precisely its spatial part. ψ ( k ) we call the wavefunction in momentum representation. For the expectation value of the momentum we write ∞
〈 pˆ 〉 = — 〈φkφ〉 =
∫
–∞
∞
φ∗ ( k ) pˆ φ ( k ) dk = – i—
∂
∫ ψ∗ ( x ) ∂ x ψ ( x ) d x
(3.7)
–∞
The important message in (3.7) is that the result of calculating an expectation value does not depend on the representation of the wavefunction. Note that when representing wavefunctions in position space the momen∂ tum is a differential operator pˆ = i—  . This implies that the momentum ∂x operator and the position operator do not commute, i.e., applying the chain rule for differentiation we see that ( pˆ x xˆ – xˆ pˆ x )ψ ( x ) = – i—ψ ( x )
(3.8)
holds. In other words, it makes a difference whether pˆ x xˆ or xˆ pˆ x is applied to ψ ( x ) and it does not give the same result. (3.8) is called the commutator of the operators pˆ x and xˆ . If operators do not commute, i.e., the commutator has a nonzero value, this means that the respective physical quantities cannot be measured simultaneously with arbitrary precision.
100
Semiconductors for Micro and Nanosystem Technology
Quantum Mechanics of Single Electrons
Uncertainty Principle
This leads directly to the uncertainty principle for operators, which is one of the central points of quantum theory that has always been subject of many discussions from the moment of its formulation. For the gaussian wavefunction (3.5) centered at x 0 = 0 , the variances of the particles position and momentum are ∞
〈 ( ∆xˆ ) 2〉
1 σ = ( 2π ) 1 / 2
∫
x2 exp – 2 x 2 dx = σ 2 2σ
(3.9)
–∞
and ∞
〈 ( ∆ pˆ ) 2〉
2 = hσ π
h2
∫ exp ( –k σ )k dk = 4σ 2
2
2
2
(3.10)
–∞
respectively. OneDimensional System
Take a onedimensional system with wavefunction ψ ( x ) in its spatial representation, that is deﬁned in the entire interval ( – ∞, ∞ ) . Suppose that 〈 xˆ 〉 = 0 and 〈 pˆ 〉 = 0 hold. This assumption is not necessary but taking arbitrary values for the expectation values of position and momentum only makes the calculation more complicated without increasing the understanding. The relation ∞
∫
αxψ +
dψ 2 dx dx
–∞
=
∞
∫
–∞
(3.11)
∗ dψ dψ∗ dψ α 2 x 2 ψ 2 + x dψ ψ + xψ∗  +   dx ≥ 0 dx dx dx dx
is evident since the square modulus is positive in ( – ∞, ∞ ) . Here α is an arbitrary real constant. Talking into account (3.1), (3.3) and (3.7) and performing integration by parts we obtain 1 α 2 〈 ( ∆xˆ ) 2〉 – α +  〈 ( ∆ pˆ ) 2〉 ≥ 0 —
Semiconductors for Micro and Nanosystem Technology
(3.12)
101
The Electronic System
This inequality is to hold for arbitrary real α . Thus, —2 〈 ( ∆xˆ ) 2〉 〈 ( ∆ pˆ ) 2〉 ≥ 4
(3.13)
must hold. (3.13) is called the Heisenberg uncertainty principle. Heisenberg derived it in 1925, and it gave rise to the creation of a new physical discipline called quantum mechanics. The simple signiﬁcance is that the product of the variances of position and momentum has a minimum, which is — 2 ⁄ 4 . Since it clearly derives from the commutator relations its physical interpretation is that position and momentum may not be determined by measurement with arbitrary precision. Note that (3.13) only gives a lower limit. Now, turning back to the example of a gaussian wavefunction we see that it is a function, we see that it is a function fulﬁlling (3.13) exactly with the “=”sign. Thus we call it a state of “minimal uncertainty”.
3.1.2 The Schrödinger Equation The quantitative description of wavefunctions was given by Erwin Schrödinger in 1924. An example of a classical wave equation is a partial differential equation of second order in space and time. The corpuscular nature of the light ﬁeld as discovered by Einstein relates the energy E of the photon to the angular frequency of the electromagnetic wave by E = —ω , while its momentum is given by p = —k . The assumption of De Broglie for those relations to hold also for particles together with E = — 2 k 2 ⁄ ( 2m ) led Schrödinger to take an equation of ﬁrst order in time. This equation of motion must read ∂ —2 i— Ψ ( x, t ) = –  ∇2Ψ ( x, t ) ∂t 2m
(3.14)
which is a partial differential equation of ﬁrst order in time and second order in space. Note the fact that an imaginary coefﬁcient of the time derivative turns (3.14) into a wave equation. The spatial derivative of sec
102
Semiconductors for Micro and Nanosystem Technology
Quantum Mechanics of Single Electrons
ond order with its coefﬁcient Tˆ = – — 2 ⁄ ( 2m ) ∇ 2 is, according to the discussion about the momentum operator in 3.1.1, the operator of the kinetic energy in a spatial representation. The equation of motion for the Schrödinger ﬁeld Ψ in a potential is given by ∂ ˆ Ψ ( x, t ) i— Ψ ( x, t ) = ( Tˆ + U ( x ) )Ψ ( x, t ) = H ∂t
(3.15)
ˆ = Tˆ + U ( x ) is called the Hamilton operator of a closed system if H U ( x ) does not depend explicitly on the time variable t . This means that the solution of the system described by (3.15) is invariant under translations in time. Wavefunctions for which the energy has a speciﬁc value are called stationary states. We denote them as Ψ n and call them eigenfunctions of the Hamilton operator. All of them follow the equation ˆ Ψ n = E n Ψ n , which is called the eigenvalue equation for the Hamilton H operator. The total of eigenfunctions and eigenvalues is called the spectrum of the Hamilton operator. In this case we integrate (3.15) in time, which gives i Ψ n = exp –  E n t ψ n ( x ) —
(3.16)
where the function ψ n depends only on the coordinates. (3.16) gives the time dependence of the wavefunction, while the spatial dependence and the energy of the eigenstate must be found solving the respective eigenvalue problem resulting inserting (3.16) into (3.15) ˆ ψn( x ) = Enψn( x ) H Quantum Numbers
(3.17)
The numbers n counting the different energies are called quantum numbers. The stationary state with the lowest energy we call the ground state. We recall some technical aspects from linear algebra:
• For every discrete eigenvalue problem, there might be multiple eigenvalues which results in different eigenvectors for the same eigenvalue.
Semiconductors for Micro and Nanosystem Technology
103
The Electronic System
• With the knowledge of the whole energy spectrum, i.e., all the eigenvalues and eigenvectors that form a complete basis set, we may represent an arbitrary vector as an expansion into the eigenvectors. Ψ ( x, t ) =
i
∑ a exp – — E t ψ ( x ) n
n
n
(3.18)
n
• The eigenvectors are orthogonal ( 〈ψ nψ m〉 = δ nm ). This means that the “scalar product” as deﬁned for the wavefunctions through (3.1) is zero for n ≠ m and one for n = m . The square moduli a n 2 denote the probability of ﬁnding the system in a special eigenstate. The spatial probability distribution is given by Ψ n 2 = ψ n 2 , it does not depend on time, which also holds for the expectation values of operators that do not depend explicitly on time. All those quantities are called conserved quantities. All conserved quantities commute with the Hamilton operator, i.e., we may measure them at the same time we measure the energy of the system. Nevertheless, they may not always give the same result for their expectation values and seem not to be uniquely deﬁned in the case where there exist multiple energy eigenvalues. Thus we need to know more about the system than only the energy of the respective state or, in other words, in some situations the energy spectrum does not contain enough information about the system to be described uniquely. When talking about conserved quantities, we may ask for the probability ﬂux through the surface Γ of a ﬁnite volume Ω , i.e., the continuity equation for the probability density in the same way as it exists for the charge density in electrodynamics. For this purpose, we integrate the probability density (3.2) on the entire volume Ω and take its time derivative: ∂ ( Ψ 2 dV ) = ∂t
∫
Ω
∂ψ ∗
∂ψ
 ψ + ψ∗  dV ∫ ∂t ∂t
Ω
i ˆ Ψ∗ – Ψ∗ H ˆ Ψ ) dV ) =  ( ( ΨH —
∫
Ω
104
Semiconductors for Micro and Nanosystem Technology
(3.19)
Quantum Mechanics of Single Electrons
where we used (3.15) and the fact that for the Hamilton operator ˆ = H ˆ ∗ holds. We use H — 2 ˆ = – ∇ + U ( x ) H 2m
(3.20)
Ψ∇ 2 Ψ∗ – Ψ∗ ∇ 2 Ψ = ∇ ( Ψ∇Ψ∗ – Ψ∗ ∇Ψ )
(3.21)
and
which yields a continuity equation of the form d Ψ 2 dV = – ∇ j dV dt
∫
Ω
∫
(3.22)
Γ
where Γ is the surface of the region Ω . Here j is the current density vector, which is identiﬁed by 1 i— j =  ( Ψ∇Ψ∗ – Ψ∗ ∇Ψ ) =  ( Ψ pˆ ∗ Ψ∗ – Ψ∗ pˆ Ψ ) 2m 2m
(3.23)
Box 3.1. The Gauss Theorem. The Gauss Theorem. Consider a vector ﬁeld A ( r ) and a volume element V with a closed surface S V . The normal vector n of the surface points outward the volume element. Then we have the following relation between the surface integral and the volume integral of the vector ﬁeld
°∫ S
V
Ads =
∫ ∇ A dV
(B 3.1.1)
V
This is called the Gauss theorem. Due to this equation the properties of the ﬁeld inside V especially its sources are related to its properties at the surface – especially its ﬂux.
Current Density
This is also true for situations where the volume is a non simply connected region, i.e., there may be holes in V . In components we formulate the theorem for arbitrary dimensions D as follows
°∫ d si …
SV
=
∂
∫ dV ∂ x i …
(B 3.1.2)
V
where the dots are to be replaced by a vector ﬁeld, or even a scalar ﬁeld, while i = 1, 2, …, D . This means that the surface integral is related to the volume integral of the derivative of the ﬁeld.
This is the current density of probability or simply the current density. For a given electronic system its expectation value multiplied by the unit charge corresponds to a measurable electrical current density.
Semiconductors for Micro and Nanosystem Technology
105
The Electronic System
Gauss theorem
Applying the Gauss theorem, (see Box 3.1), we see that d Ψ 2 dV = – j dS dt
∫
∫
(3.24)
holds. (3.24) has a very simple interpretation: the change of probability density with time in the volume Ω is caused by the ﬂux through the surface Γ .
3.2 Free and Bound Electrons, Dimensionality Effects Another more sophisticated point is the fact that the energy spectrum may show a both discrete and a continuous part. This leads us to the following question: How does the spectrum depend on the imposed boundary conditions? To determine ﬁnally the functional form of the wavefunction, we need information about these boundary conditions that the electronic system has to fulﬁll. The resulting spectrum of observables will be discrete, continuous or mixed and allows us to talk about its dimensionality [3.1], [3.2].
3.2.1 Finite and Inﬁnite Potential Boxes The OneDimensional Potential Box
The simplest case to study appears to be the onedimensional potential box with ﬁnite potential. The physical interpretation of its solution and boundary conditions, and the transition to inﬁnite potential walls, are very instructive. Given the potential 0, x ∈ [ 0, a ] U ( x) = U 0 , x ∉ [ 0, a ]
106
Semiconductors for Micro and Nanosystem Technology
(3.25)
Free and Bound Electrons, Dimensionality Effects
the spectrum of the Hamiltonian will have both discrete and continuous eigenvalues. The onedimensional time independent Schrödinger equations read 2m d2 2Ψ + 2EΨ = 0 , for x ∈ [ 0, a ] — dx
(3.26a)
2m d2 2Ψ + 2 ( E – U 0 )Ψ = 0 , for x ∉ [ 0, a ] — dx
(3.26b)
The Schrödinger equation, as given in (3.26a) and (3.26b), are differential equations of second order. To ﬁnd their solutions we must provide additional information, i.e., conditions to hold in the physical domain Ω or on its boundary.
• The probability density must be smooth at x = 0 and x = a , and so must be the wavefunction. This is because there are no sources or sinks for the probability density, i.e., there is neither particle creation nor destruction going on, i.e., (3.24) holds: lim ( Ψ ( +ε ) – Ψ ( – ε ) ) = 0 and lim ( Ψ ( a+ε ) – Ψ ( a – ε ) ) = 0
ε→0
ε→0
• For the same reason the ﬂux of probability density must also be continuous at the interface and so d d lim  Ψ ( +ε ) –  Ψ ( – ε ) = 0 and dx
(3.27a)
d d lim  Ψ ( a+ε ) –  Ψ ( a – ε ) = 0 . dx
(3.27b)
ε → 0 dx
ε → 0 dx
The trial function for the solution of (3.26a) and (3.26b) is ψ = const. ⋅ exp ( λx ) . Inserting this, we obtain for λ – 2mE  , for x ∈ [ 0, a ] λ = ± ik = ± —2
(3.28a)
2m ( U 0 – E )  , for x ∉ [ 0, a ] λ = κ = ± —2
(3.28b)
Semiconductors for Micro and Nanosystem Technology
107
The Electronic System
Bound Electrons, Free Electrons
There are harmonic solutions for E > U 0 , because the radicands in (3.28a) and (3.28b) are always negative in this case and thus the solution for λ is imaginary. Electrons in these states are called unbound electrons or free electrons. Their λ is the well known wavevector k and their wavefunctions do not necessarily vanish for x → ± ∞ . We shall discuss their properties together with the free electron states. For now we are interested in the solutions with energy eigenvalues E < U 0 , called bound states. Their wavefunction decays exponentially in regions I and III (see Figure 3.3). The plus sign in (3.28b) must hold for x < 0 , while the
V ( x) V0
x 0
a
Figure 3.3. Finite box potential in one dimension.
minus sign must hold for x > a . In the regions I and III we call λ = κ . Inside the box we have a harmonic solution, with wavevector k . Thus we obtain ψ I ( x ) = A exp ( κx )
(3.29a)
ψ II ( x ) = B exp ( ikx ) + C exp ( – ik x )
(3.29b)
ψ III ( x ) = D exp ( – κ x )
(3.29c)
The boundary conditions read
108
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
ψI
x=0
= ψ II
x=0
ψ I'
x=0
= ψ II '
x=0
ψ II
x=a
= ψ III
x=a
ψ II '
x=a
= ψ III '
x=a
(3.30a) (3.30b) (3.30c) (3.30d)
Inserting (3.29a)(3.29c) into (3.30a)(3.30d), we obtain a linear system of equations to determine AD: 1 –1 –1 0 ika – i ka 0 e e – e –κa κ – ik ik 0 0 ike ika – ike –i ka κe –κa
A B = 0 C D
(3.31)
A solution can only be found if the determinant of the coefﬁcient matrix in (3.31) is zero: 2κk cos ( ka ) + ( κ 2 – k 2 ) sin ( ka ) = 0 With ak = ξ we have aκ = may write (3.32) as
( 2mU 0 a 2 ) ⁄ — 2 – ξ 2 =
2ξ C 2 – ξ 2 + tan ξ = 0 C 2 – 2ξ 2
(3.32) C 2 – ξ 2 and we
(3.33)
This equation must be solved either graphically, see Figure 3.4 and Figure 3.5, or by numerical methods. A numerical solution of the discretized model for the discussed eigenvalue scenario may be counterchecked in the special case with U 0 « — 2 ⁄ ( ma 2 ) where there is exactly one bound state found with E 0 ≈ U 0 ( 1 – ma 2 ⁄ ( 2— 2 ) ) . Note that only in special limiting cases can an analytical solution be obtained easily. Usually, analytical methods end at a certain point and
Semiconductors for Micro and Nanosystem Technology
109
The Electronic System
C
ξ
2ξ C 2 – ξ 2 C 2 – 2ξ 2
– tan ξ
Figure 3.4. Graphical solution for equation (3.33). The intersection of the two expressions – tan ξ and ( 2ξ C 2 – ξ 2 ) ⁄ ( C 2 – 2ξ 2 ) , indicated by the circle, is the ﬁrst solution point. Also see Figure 3.4.
E
Figure 3.5. Change in energy E as a function of well width a , for the ﬁrst solution of equation (3.33), as given by the graphical solution (marked with a circle) in Figure 3.4.
a
have to be succeeded by numerics. Since semiconductor structures are becoming more and more complicated, there is no way of dealing with the electronic structure calculations in an analytical way. The reader may now ask why all this rather theoretical material is discussed in detail
110
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
here: simply because also the best simulation program is useless if there is no understanding of how to obtain a rough estimate of what the result has to be. We suggest implementing a simple numerical model for the calculation of 1D eigenvalue problems as is shown in Figure 3.8 for the harmonic oscillator potential. Inﬁnite Box Potential
We continue our discussion with the case where U 0 → ∞ . A simple physical argument tells us that for the energy of the system to be ﬁnite (the same holds for many other observable quantities), the wavefunction must vanish in the region where U ( x ) → ∞ , i.e., ψ ( x ) = 0 for x ≥ la and x ≤ 0 and for all t . The trial solution for the wavefunction ψ ( x ) = B exp ( ikx ) + C exp ( – ik x ) must fulﬁll the boundary condition ψ ( 0 ) = 0 and ψ ( a ) = 0 . This leads to ψ ( x ) = B sin ( kx ) , with k = ( nπ ) ⁄ a and n integer and positive starting at n = 1 . Inserting this into the time–independent Schrödinger equation (3.17) gives us the energy spectrum of the inﬁnite box potential: π2— E n = 2 n 2 , with n = 1, 2, 3, … 2ma
(3.34)
The normalized wavefunction reads ψn( x ) =
2 nπx  sin a a
(3.35)
We give another explanation to approach the inﬁnite box potential. Suppose that U 0 » — 2 ⁄ ( ma 2 ) holds. Then there will be a part of the spectrum with low energies for which the wavefunction decays on a very short length scale outside the box, i.e., the electron is completely trapped inside the box. Three– Dimensional Potential Boxes
The above results lead us immediately to the case of an electron in a threedimensional potential box. Suppose the box is a cuboid region with 0 ≤ x ≤ a , 0 ≤ y ≤ a , and 0 ≤ z ≤ a . Inside the box U ( x, y, z ) = 0 , while outside U ( x, y, z ) → ∞ . The energy spectrum looks like
Semiconductors for Micro and Nanosystem Technology
111
The Electronic System
condition for normalizing the eigenfunctions of a continuous spectrum. We have chosen the expansion coefﬁcients as φ k on purpose in order to show that the situation of the gaussian wavefunction expanded in plane waves is exactly such a case. The inﬁnitely extended momentum eigenfunctions describe ideal situations having an exact value for the momentum of the electron. According to the Heisenberg principle, allowing the transition for the momentum variance to vanish, this yields an inﬁnite variance of its position such that their product is larger than — 2 ⁄ 4 . This can only be a hand–waving argument to visualize the situation. Nevertheless, it gives a feeling for the consistency problems arising. The gaussian wavefunction, in contrast, is an excellent example of a more realistic situation. Its interpretation is that of a moving electron having an expectation value of momentum and position with their respective variances in accordance with the Heisenberg principle. It is a more realistic situation because the arrival of electrons at a certain position may be measured and it coincides with an event of the measuring instrument. It is not possible here to go deeper into this subject but nevertheless we want to draw readers’ attention to the literature on the problem of measurement in quantum mechanics. The Continuous Spectrum of the Quantum Box
Suppose E > U 0 in (3.28a) and (3.28b). Then the solutions in the three regions I, II and III read ψ I ( x ) = a 1 exp ( ik I x ) + a 2 exp ( – ik I x )
(3.42a)
ψ II ( x ) = b 1 exp ( ik II x ) + b 2 exp ( – ik II x )
(3.42b)
ψ III ( x ) = c 1 exp ( ik III x ) + c 2 exp ( – ik III x )
(3.42c)
where we have k I , III = 2m ( E – U 0 ) ⁄ — and k II = 2mE ⁄ — . In Figure 3.3 a wavefunction for a free electron is indicated. The larger kinetic energy in the box region yields a larger wavevector k and thus a wavefunction oscillating faster in space.
114
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
3.2.3 Periodic Boundary Conditions A practical approach to set boundary conditions would be to have an inﬁnite box potential with a large extension from x = 0 to x = L forcing the wavefunction to vanish on the boundaries. This seems to be artiﬁcial: because of the vanishing wavefunction it is hard to imagine how electrons get into or out of the sample. There is another way of introducing boundary conditions for free electrons in one dimension that requires the wavefunction to be periodic, i.e., ψ ( 0 ) = ψ ( L ) . This allows us to have plane wave solutions for the Schrödinger equation, that are normalized to the length L : ψ ( x ) = ( L ) –1 / 2 exp ( ikx )
(3.43)
Applying periodic boundary conditions the wavevector is restricted to 2πn k = L
(3.44)
Taking L = N ⋅ a , i.e., in multiples of the atomic spacings, there are N discrete values for k to fulﬁll the periodic boundary condition.
3.2.4 Potential Barriers and Tunneling Let us discuss the situation inverse to that given in Figure 3.3, i.e., a potential of the form U , x ∈ [ 0, a ] U ( x) = 0 0, x ∉ [ 0, a ]
(3.45)
(see also Figure 3.6). We insert the potential (3.45) into the Hamiltonian. Again we choose ψ = const. ⋅ exp ( λx ) as the trial solution. Thus we obtain – 2mE λ = ± i k I = ±  , for x ∉ [ 0, a ] —2
Semiconductors for Micro and Nanosystem Technology
(3.46a)
115
The Electronic System
V ( x)
V0
Figure 3.6. Barrier potential and sketched real part of a harmonic wavefunction hitting the barrier with energy E = V 0 ⁄ 2 , i.e., smaller than V 0 .
0
a
2m ( U 0 – E )  , for x ∈ [ 0, a ] λ = ± k II = ± —2
x
(3.46b)
There are no bound states in this case because the region where harmonic solutions exist is inﬁnite. The states with energies E > U 0 show the inverse behavior as for the box potential (3.25). This is indicated in Figure 3.6. Remember that there exist solutions that decay exponentially inside the barrier and extend to inﬁnity on either side of the barrier for E < U0 . We analyze this situation further. Consider a free electron impinging the barrier from region I to have a deﬁnite wavevector k I . Thus our trial functions read ψ I ( x ) = a 1 exp ( ik I x ) + a 2 exp ( – ik I x )
(3.47a)
ψ II ( x ) = b 1 exp ( k II x ) + b 2 exp ( – k II x )
(3.47b)
ψ III ( x ) = c 1 exp ( ik I x ) + c 2 exp ( – ik I x )
(3.47c)
We assume the impinging wave to have unit amplitude ( a 1 = 1 ) and further that there is no wave travelling from region III towards the barrier ( c 2 = 0 ). Note that k I = k III . On either side of the barrier the conditions for the continuity of the wavefunction ψ and its spatial derivative
116
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
dψ ⁄ dx must be fulﬁlled. This yields a system of four equations that determine the four remaining coefﬁcients a 2, b 1, b 2, and c 1 . The solutions reads a 2 = ( exp ( ik II a ) – exp ( – ik II a ) ) ( k I2 – k II2 )D –1
(3.48a)
b 1 = 2 exp ( i ( k I – k II )a )k I ( k I + k II )D –1
(3.48b)
b 2 = 2 exp ( i ( k I + k II )a )k I ( k II – k I )D –1
(3.48c)
c 1 = 4k I k II D –1
(3.48d)
with D = exp ( ik I a ) [ exp ( ik II a ) ( k I – k II ) 2 – exp ( – i k II a ) ( k I + k II ) 2 ] .In Figure 3.6 the real parts of the different superposing wavefunctions are sketched for values E > U 0 and E < U 0 . There are several remarkable features to discuss: Reﬂection, Transmission and Tunneling
• c 1 is nonzero for E < U 0 . In this case the particle behaves rather wavelike. This is very similar to a lightwave going through materials with different refractive index. There is always a reﬂected and a transmitted part, i.e., a 2 ≠ 0 and c 1 ≠ 0 .
• For E > U 0 the situation changes. We ﬁnd resonances for the transmission at k II a = n ⋅ π with n an integer. There is no reﬂection in this case, whereas there is always a transmitted part, i.e., c 1 ≠ 0 . Reﬂection and transmission are not uniquely deﬁned by the amplitudes of the partial waves alone. Therefore, we deﬁne the reﬂexivity R as the quotient of reﬂected and incoming current density; the quotient of transmitted and incoming current density we call the transmitivity T : R = a2 2 ⁄ a1 2 = a2 2
(3.49a)
T = c1 2 ⁄ a1 2 = c1 2
(3.49b)
In the case where there is neither creation nor destruction of particles, R + T = 1 must hold. In Figure 3.7 T is shown with increasing energy E of the incoming wave. There are well deﬁned resonances where the
Semiconductors for Micro and Nanosystem Technology
117
The Electronic System
T 1.0
0.5
Figure 3.7. Transmission probability T versus E . E is measured in multiples of V 0 .
E 1
2
3
4
whole incoming wave is transmitted. T also shows pronounced minima for E ≥ V 0 , which one does not expect in a classical behavior.
3.2.5 The Harmonic Oscillator In Section 2.4.1 the normal modes of vibration for a lattice were introduced. It has been shown that in a ﬁrst approximation the Hamilton function of the total lattice vibration is a sum of noninteracting harmonic oscillators. The quantization of the lattice vibrations has been presumed in 2.4.1 to explain the discrete nature of phonons. The intercommunity with electrons crops up due to the form of the potential energy. Harmonic Oscillator Potential
U = mω 2 q 2 ⁄ 2 is the potential energy of a linear harmonic oscillator in one dimension. The Hamiltonian for a particle moving in such a potential
reads pˆ 2 m 2 2 ˆ = Tˆ + U ˆ = H  +  ω q 2m 2
(3.50)
The potential energy U goes to inﬁnity as q → ± ∞ . Therefore, the particles’ wavefunction must go to zero for q → ± ∞ . The resulting spectrum of the Hamiltonian will be discrete, with energy eigenvalues E n and the respective eigenfunctions Ψ n = exp ( – ( i ⁄ — ) E n t ) ψ n ( q ) . The variable q denotes the amplitude of the oscillator spring or the position of the
118
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
electron in the harmonic potential. This is why both phenomena may be described in the same way. We describe the oscillator in the qrepresentation. This means that the momentum operator is given by pˆ = – i— d ⁄ dq , and the commutator is pˆ qˆ – qˆ pˆ = – i— . The time–independent Schrödinger equation reads —2 d 2 m 2 2  2 +  ω q ψ ( q ) = Eψ ( q ) –  2 2m dq With the coordinate transformation q =
(3.51)
— ⁄ ( mω ) ξ (3.51) reads
—ω d 2  – 2 + ξ 2 ψ ( ξ ) = Eψ ( ξ ) 2 dξ
(3.52)
The operator in braces in (3.52) has the form a 2 – b 2 = ( a – b ) ( a + b ) and thus may be written as 1 d   + ξ dξ 2
—ω + 2
—ω d 2 1 d  – 2 + ξ 2 = —ω  –  + ξ 2 dξ dξ 2 b+
b
(3.53)
With the deﬁnitions of the operators b + and b as given by the underbraces in (3.53) and shifting the zero point of the energy according to E′ = E – —ω ⁄ 2 , the Schrödinger equation reads —ω b + b ψ = E′ψ
(3.54)
This simple form allows us to calculate the wavefunctions very easily. We calculate the commutator of b + and b , which gives [ b, b + ] = bb + – b + b = 1
(3.55)
Take the ground–state function ψ o that has the lowest energy eigenvalue E o′ . Let the operator b act on both sides of (3.54)
Semiconductors for Micro and Nanosystem Technology
119
The Electronic System
—ω bb + b ψ o = E o′ bψ o
(3.56)
which gives with (3.55) —ω ( 1 + b + b ) bψ o = E o′ bψ o
(3.57)
—ω b + b bψ o = ( E o′ – —ω )bψ o
(3.58)
or
(3.58) means that there is a ground state ψ o′ = bψ o with an even smaller energy than E o′ . This is contradictory to the presupposition that ψ o be the ground state. Even if the ﬁrst choice of ψ o had not been the right ground state, repeated execution of the operation in (3.56) would lead us to an energy eigenvalue E o′ → – ∞ . This cannot be, since the potential energy is bound, with its minimum at U = 0 . On the other hand, (3.56) is a valid equation with a valid operation. Thus the only solution is that bψ o = 0 . Inserting the deﬁnition of the operator b given in (3.53) yields d  + ξ ψ o ( ξ ) = 0 dξ
(3.59)
1 ξ2  ⋅ exp –  ψ o ( ξ ) = 1 ⁄ 4 2 (π)
(3.60)
with the solution Ground–State Oscillator Wavefunction
bψ o = 0 implies that the l.h.s. of (3.54) is zero for the ground–state wavefunction and thus we have E o′ = 0 . This gives us the ground state energy E o = ( —ω ⁄ 2 ) . We perform the same operation as in (3.56), now letting b + act on the Schrödinger equation for the ground state, which gives —ω b + b + b ψ o = E o′ b + ψ o
120
Semiconductors for Micro and Nanosystem Technology
(3.61)
Free and Bound Electrons, Dimensionality Effects
Considering the commutator for the operators b + and b we obtain —ω b + b b + ψ o = ( E o′ + —ω )b + ψ o
(3.62)
Obviously ψ 1 = b + ψ o is an eigenvector of the operator —ω b + b with eigenvalue E o′ + —ω . Number Operator
Excited State WaveFunction
Repeating this procedure n times we obtain the nth eigenvector ψ n with eigenvalue E n′ = n—ω (remember E o′ = 0 ). Thus we have E n = ( n + 1 ⁄ 2 )—ω . The quantum number n characterizes the oscillator and is the eigenvalue of the quantum number operator b + b . The normalized wavefunction for an arbitrary excited state with quantum number n reads 1 1 ψ n =  ( b + ) n ψ o = n〉 =  ( b + ) n 0〉 n! n!
(3.63)
where n〉 indicates the Dirac notation of a quantum state with n excited oscillator quanta and 0〉 describes the oscillator vacuum with no quanta present. Hence we have, from b + , the number of oscillator quanta incremented by one, and applying on n〉 results in b + n〉 =
n + 1 n + 1〉
(3.64)
n n – 1〉
(3.65)
while applying b yields b n〉 = Bosons
Note that the oscillator quantum number can be arbitrarily large for a given state. This is the case for particles that follow Bose statistics (see Chapter 5) and therefore these particles are called bosons.
Minimum Uncertainty
The quantum mechanical harmonic oscillator states apply for the description of various different phenomena and not only in semiconductors. In addition, it has a very important property because the ground–state wavefunction fulﬁlls the equality in (3.13), i.e., the wavefunction is a quantum state of minimum uncertainty. This is easily shown by calculating the Semiconductors for Micro and Nanosystem Technology
121
The Electronic System
variances as (3.9) and (3.10). We recall the transformation q = — ⁄ ( mω ) ξ , thus we have the momentum operator given by pˆ = – i— d ⁄ dq = ( mω ) ⁄ — d ⁄ dξ . Since the potential is symmetric about q = 0 we have 〈 qˆ 〉 = 0 and 〈 pˆ 〉 = 0 . We calculate 〈 qˆ 2〉 and 〈 pˆ 2〉 : ∞
〈 qˆ 2〉
1 — 1 — ξ 2 – ξ2 ξ 2 exp – =   dξ =  exp 2 2 2 mω mω ( π ) 1 ⁄ 2
∫
(3.66a)
∞
∞
〈 pˆ 2〉
1 ξ2 —mω ξ2 d2  exp –  2 exp –  dξ = = – —mω 1 ⁄ 2 2 2 2 dξ (π)
∫
(3.66b)
∞
and thus their product yields —2 〈 ( ∆xˆ ) 2〉 〈 ( ∆ pˆ ) 2〉 = 〈 pˆ 2〉 〈 qˆ 2〉 = 4
(3.67)
A numerical treatment of the harmonic oscillator problem together with the plots of eigenfunctions is given in Figure 3.8. 25 20
Figure 3.8. A harmonic potential is indicated by the gray shaded background. The black lines to the left show the symmetric eigenmodes of this potential, aligned with their respective energy eigenvalues. The black lines to the right are the antisymmetric eigenmodes, similarly aligned.
122
15 12.9466 10.9617 10
8.9743 6.9843
5
4.9919 2.9969 0.9994
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
3.2.6 The Hydrogen Atom The paradigm for the electronic states of a central symmetric potential is the hydrogen atom since it consists of one proton in the nucleus surrounded by one electron. It helps in understanding the principle of electronic states of atoms which is similar to the electronic states of defects and traps for electrons in the semiconductor or even helps to understand the formation of a band structure. We shall not go into details of the derivation but we shall have a closer look at the form of the electronic states. Coulomb Potential
The Coulomb potential of the proton is spherically symmetric in three dimensions, which means that it depends only on the distance r of the symmetry center U ( r ) = – e 2 ⁄ r (e is the unit charge). The best choice to tackle the problem is spherical coordinates, with the radius vector r given by its modulus r , the polar angle φ and the azimutal angle θ . The Hamilton operator thus reads —2 e2 H = –  ∇ 2 – r 2µ
(3.68)
To solve the Schrödinger equation we must write the ∇ 2 in spherical coordinates, which reads ∂ 1 ∂2 1 ∂ 1 1 ∂ ∂ ∇ 2 = 2 r 2 + 2  sin θ +  ∂ θ sin 2 θ ∂φ 2 r ∂r ∂r r sin θ ∂ θ
(3.69)
Inserting (3.69) together with (3.68) and solving the respective Schrödinger equation is beyond the scope of this book. We restrict the discussion to an interpretation of the electronic wavefunction and an illustration of the atomic orbitals. The common approach to calculate the bound electronic states of the hydrogen atom (energy E < 0 ) starts with a product trial function for the wavefunction ψ ( r ) = R ( r )Y ( θ, φ ) . Then the Schrödinger equation separates into two eigenvalue problems, one for the radial motion ( R ( r ) ) and one for the angular motion ( Y ( θ, φ ) ). The solutions of the angular
Semiconductors for Micro and Nanosystem Technology
123
The Electronic System m
part are the spherical harmonic functions Y l ( θ, φ ) (see Table 2.2). The radial functions are R ( r ) = R n, l ( r ) ⁄ r , where the R n, l ( r ) follow a differential equation of Laguerre type, and are shown in Figure 3.9• for dif
1
1
1
5
1
1
1
Figure 3.9. The radial wavefunction R n, l ( r ) for different n and l .
ferent ( n, l ) . The wavefunction ψ n, l, m ( r, θ, φ ) (see Table 3.1) has three integer parameters:
• n : the quantum number of radial motion, • l = 0, 1, …, n – 1 : the ﬁrst quantum number of angular motion, • m = – 1, …, 1 : the second quantum number angular motion (note that m is an integer, not to be confused with the mass of the electron).
124
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
Table 3.1. The wavefunction ψ n, l, m ( r, θ, φ ) . n
l
ψ n, l, m ( r, θ, φ )
m
1
0
0
γ2  ⋅ π
2
0
0
γ2 ⋅ π
2
1
0
γ2 ⋅ π
2
1
±1
γ2 2π
3
0
0
γ2 3 π
3
1
0
3
1
±1
γ2 3π
3
2
0
3
2
±1
γ2 3π
3
2
±2
γ2 2 3π
Degenerate Spectrum
3⁄2
exp ( – r )
3⁄2
(1 – r ⁄ 2) ⋅
exp ( – r ⁄ 2 )
3⁄2
r⋅
exp ( – r ⁄ 2 )
cos θ
3⁄2
r
exp ( – r ⁄ 2 )
sin θe ±iφ
3⁄2
( 2 – 2r + 2r 2 )
exp ( – r ⁄ 3 )
( 2 – r ⁄ 3 )r
exp ( – r ⁄ 3 )
cos θ
( 2 – r ⁄ 3 )r
exp ( – r ⁄ 3 )
sin θe ±iφ
γ2 3 2π
r2
exp ( – r ⁄ 3 )
( 3cos 2 θ – 1 )
3⁄2
r2
exp ( – r ⁄ 3 )
cos θ sin θe ±iφ
r2
exp ( – r ⁄ 3 )
sin 2 θe ±2iφ
3⁄2
2γ 2 3π 3⁄2
3⁄2
3⁄2
Each quantum state represents an atomic energy level E n, l, m that is typical for the hydrogen atom, i.e., typical for the potential energy given in the Hamiltonian (3.68). There are nevertheless sets of quantum numbers, i.e., well distinguishable wavefunctions, that have the same energy eigen
Semiconductors for Micro and Nanosystem Technology
125
The Electronic System
value. This multiple eigenvalue phenomenon is well known from linear algebra, and is called degeneracy. All energies of the hydrogen spectrum with equal quantum number n are degenerate. Note that the Pauli principle is still valid, because the wavefunctions are different. This degeneracy can be lifted by adding a potential that acts on the respective wavefunctions differently for different quantum numbers. In fact, nature provides us with such additional interaction potentials and an exact measurement of the spectrum a hydrogen atom does not show theses degeneracies. The conclusion is that our model is too simple. Nevertheless, it explains the principles that the electronic system of atoms follows. One major incompleteness is that for manyelectron systems the Coulomb interaction between the electrons must be taken into account. This makes the Schrödinger equation highly nonlinear and thus other techniques including numerics must be used. Moreover, if we want to understand the formation of crystal symmetry by just putting atoms together, this interaction is responsible for the details in the electronic band structure. Scattering
So far we have only dealt with the bound states of the atom and an electron occupying one of them. There is no dynamics in this picture, because there is no process represented by an interacting potential that might change this static situation. Suppose a free electron collides with the atom, then there are several possibilities:
• the electron gets trapped and subsequently occupies a quantum state of the atom, it emits a photon carrying away the energy difference between the free state and the bound state;
• it is scattered and moves on with a different wavevector, there is a momentum transfer and an energy transfer between the electron and the atom;
• the transferred energy excites a bound electron already occupying a quantum state, the free electron moves on with a lower kinetic energy, the bound electron either occupies an excited state higher in energy, or even leaves behind an ionized atom moving freely;
126
Semiconductors for Micro and Nanosystem Technology
Free and Bound Electrons, Dimensionality Effects
• the excited electron bounces back to its ground state, emitting a photon. All those processes require the transitions of electrons between different electronic states. The scenario described above is what happens in a gas discharge lamp. The analogous process can be found in the conduction band of a semiconductor where an electron is hitting a defect atom that has a spectrum of localized electronic states below the conduction bandedge. The energy scale is of course one order of magnitude lower and there are additional degrees of freedom to which the excess energy of the electron may be transferred, e.g., phonons. The quantum mechanical description of the electron as given above focused on the stationary states of the electrons. Now the time dependence of the Schrödinger equation has must be exploited.
3.2.7 Transitions Between Electronic States The superposition of the time–dependent solutions of the Schrödinger equation (3.16) gives the general form of the wavefunction with arbitrary initial conditions Ψ 0 ( x, t ) =
∑ c exp ( –iω t )ψ ( x ) n
n
n
(3.70)
n
where ω n = E n ⁄ — and the ψ n ( x ) in (3.70) are the solution of the stationary eigenvalue problem ˆ 0ψn = Enψn H
(3.71)
The coefﬁcients c n are determined by the initial condition, i.e., c n = 〈ψ n ( x )Ψ 0 ( x, 0 )〉 . The superscript 0 of the wavefunction and the subscript 0 of the Hamiltonian indicate the unperturbed stationary problem.
Semiconductors for Micro and Nanosystem Technology
127
Free and Bound Electrons, Dimensionality Effects
dc m ( t ) i—  = dt
∑V
mn c n ( t ) exp ( – iω mn t )
(3.76)
n
For the following we assume that the perturbation is switched on instantaneously at t = 0 and is subsequently constant. Then the c m are given at t = 0 by the initial condition. We choose c k ( 0 ) = 1 and c n ( 0 ) = 0 for n ≠ k . For very short times after t = 0 the situation has not changed very much so that we insert the initial condition in (3.76): dc m ( t ) i—  = V mk c k ( 0 ) exp ( – iω mk t ) = V mk exp ( – iω mk t ) dt
(3.77)
(3.77) can be easily integrated to give t
i c m ( t ) = –  V mk exp ( – iω mk t′ ) dt′ —
∫ 0
(3.78)
1 = –  V mk ( exp ( – iω mk t ) – 1 ) —ω mk The change in the probability of ﬁnding the system in a state m is given by c m ( t ) 2 . This is the squared modulus of (3.78), which reads sin ( ω mk t ⁄ 2 ) 4 c m ( t ) 2 = 2 V mk 2 2 — ω mk Transition Rate
(3.79)
(3.79) is the probability density of ﬁnding the system at time t in ψ m if it has been found in ψ k at time t = 0 . The transition rate from k to m is given by cm ( t ) 2 Γ mk = t
(3.80)
sin ( ω mk t ⁄ 2 )  → πt  δ ( ω mk ) lim 2 ω mk 2 t→∞
(3.81)
In the long time limit
Semiconductors for Micro and Nanosystem Technology
129
The Electronic System
When the impact of the switched on interaction is over we obtain 2π Γ mk = 2 V mk 2 δ ( ω mk ) —
(3.82)
(3.82) is a very important result, called the Fermi golden rule. The transition rate from state k to m is determined by the squared matrix element of the V mk of the perturbing potential, where the deltafunction δ ( ω mk ) ensures that the energy is conserved. The approach of constant perturbation in this section can be extended to potentials which vary arbitrarily in time. We will not go into detail but rather explain the result. Let V ( ω, t ) = V 0 exp ( ± ωt ) be a perturbation varying with a ﬁxed frequency ω and an amplitude V 0 . Then the transition rate becomes 2π Γ mk = 2 V mk 2 δ ( ω mk ± ω ) —
(3.83)
The difference between (3.83) and (3.82) is that the energies E m and E k of the initial and ﬁnal states differ now by —ω , which is the energy of the special perturbation mode with frequency ω . We already know that electrons couple to periodically oscillating phenomena such as phonons and electromagnetic waves. Hence, (3.83) will be the basis for describing the scattering events that electrons in a conduction band of a semiconductor experience.
3.2.8 Fermion number operators and number states In the same manner as for the harmonic oscillator we represent the quan+ tum state of a fermion by means of a creation operator c and a destruction operator c using the Dirac notation. Deﬁning a fermion vacuum 0〉 we have +
c λ 0〉 = λ〉
130
Semiconductors for Micro and Nanosystem Technology
(3.84)
Free and Bound Electrons, Dimensionality Effects
for an electron placed in speciﬁc state λ . For the reverse operation we have c λ λ〉 = 0〉
(3.85)
where an electron has been moved out of the state λ . We must take into account that only one fermion may occupy a quantum state that is uniquely deﬁned by its quantum numbers λ . Therefore, trying to put another electron in λ must yield a zero eigenvalue + 2
( c λ ) λ〉 = 0
(3.86)
and the same must hold for twice trying to remove an electron from λ 2
( c λ ) λ〉 = 0 +
(3.87)
+
The action of the operator c λ c λ + c λ c λ on an arbitrary state β〉 yields + + ( c λ c λ + c λ c λ ) β〉 = ( 1 + 0 ) for β = λ = 1 β〉 ( 0 + 1 ) for β ≠ λ
(3.88)
which means that, regardless of whether the state λ is occupied or unoccupied, the resulting eigenvalue is 1. This leads us to the deﬁnition of the anticommutator product Anticommutator
+
+
+
{ c λ, c λ } = c λ c λ + c λ c λ = 1
(3.89)
We use curly brackets to indicate the anticommutation relation. Note the difference in the sign when compared to the commutator of oscillator + creation and destruction operators (3.55). c λ c λ = n is still the correct number operator. In the case of fermions, the number operator’s eigenvalues are either 1 or 0 and indicate whether a particle in the respective state is present or not.
Semiconductors for Micro and Nanosystem Technology
131
The Electronic System
3.3 Periodic Potentials in Crystal Lattice periodic structures create a very special situation for the electrons. Thus the properties of electrons in such kinds of potentials are different from those of a free electron [3.3]–[3.5].
3.3.1 The Bloch Functions Symmetry
A perfect crystal has a given periodicity. The special property of the electronic potential V is that it has exactly the same periodicity, i.e. V ( x + l) = V ( x)
(3.90)
where l is a arbitrary lattice vector as discussed in Chapter 2. We write (3.90) as T ( l )V ( x ) = V ( x + l ) = V ( x ) , where we used the translation operator T ( l ) , that transforms a function to its value at the place shifted by the lattice vector l from the input. Operating on the product ˆ ( x )Ψ ( x ) it is shifted by l. Since the Hamiltonian is invariant under H translation, we have ˆ ( x )Ψ ( x ) = H ˆ ( x )Ψ ( x + l ) = H ˆ ( x )T ( l )Ψ ( x ) T ( l )H
(3.91)
ˆ ( x) – H ˆ ( x )T ( l ) = 0 , i.e., T and H ˆ commute. This which means T ( l )H implies that Ψ ( x ) is also an eigenfunction of T , which means T Ψ ( x ) = λΨ ( x ) . Applying the translation operator n times yields n T Ψ ( x ) = λ n Ψ ( x ) . Since the wavefunction must be bound λ ≤ 1 . Suppose λ < 1 and replace l by –l, than again the wavefunction would not be bound in the inverse direction, thus only λ = 1 remains as a λ = exp ( ikl ) solution. Let us write and therefore Ψ ( x + l ) = exp ( ikl )Ψ ( x ) . To fulﬁl this we write the wavefunction as Ψ ( x ) = exp ( ikx )u k ( x )
(3.92)
where u k ( x ) is a lattice periodic function uk( x + l ) = uk( x )
132
Semiconductors for Micro and Nanosystem Technology
(3.93)
Periodic Potentials in Crystal
Equation (3.92) together with (3.93) is called the Bloch theorem. Thus electronic wavefunctions in a perfect crystal lattice are plane waves modulated by a lattice periodic function. We immediately recognize that the problem left is to determine the form of u k ( x ) . Therefore, we insert (3.92) into the stationary Schrödinger equation, which gives —2  ( k 2 – 2ik∇ – ∇ 2 ) + V ( x ) u k ( x ) = E k, j u k ( x ) 2m
(3.94)
We see that u k ( x ) and E k, j depend on the plane wavevector k. In addition, (3.94) allows for given k a series of eigenvalues accounted for by the index j.
3.3.2 Formation of Band Structure To construct a simple model semiconductor we take a onedimensional potential composed of barriers repeated periodically with the periodicity length L = a + b , e.g. V , x ∈ [ – b, 0 ] V ( x) = 0 0, x ∈ [ 0, a ]
(3.95)
as sketched in Figure 3.10. We insert (3.95) in (3.94) and solve the oneV ( x)
V0 –b
0
a
x
Figure 3.10. Bloch waves in a periodic crystal lattice potential.
dimensional eigenvalue problem with the ansatz
Semiconductors for Micro and Nanosystem Technology
133
The Electronic System
– i ( k – κ ) x + Be – i ( k + κ ) x ), for 0